Serving the Grease Industry Since 1933 – VOL. 82, NO. 1, MAR/APR 2018
In this issue . . . 6 The STRATCO® Contactor™ Reactor and Its Use In the Production of Calcium Sulfonate Based Greases 14 Application of New Calcium Sulfonate-Based Grease Technologies: From Laboratory to Field 32 The Typical Application of Calcium Sulfonate Complex Greases in Steel Mills 40 Novel Polymer Grease Microstructure and its Proposed Lubrication Mechanism 50 Lubricating Grease Thickeners: How to Navigate your Way through the Lithium Crisis
More Than Just a Drop in the Bucket Antioxidants VANLUBE® AZ
Friction Reducers/EP-Antiwear Agents MOLYVAN® L
VANLUBE 73 Super Plus
*MOLYVAN FEI PLUS*
*TPS™ 20,32 & 44*
Metal Deactivators *CUVAN® 303
Today’s high performance lubricants require high performance additives. Our technical staff can help you create superior products. Contact us to find out how…
Rust Inhibitors *VANLUBE RI-A
** We have over 50 lubricant additives available to meet your specific requirements.
Registered and pending trademarks appearing in these materials are those of R.T. Vanderbilt Holding Company, Inc. or its respective wholly owned subsidiaries. For complete listings, please visit this location for trademarks, www.rtvanderbiltholding.com.
hemic ilt C a rb
30 Winfield Street, P.O. Box 5150, Norwalk, CT 06856-5150 (203) 853-1400 • F: (203) 853-1452 •www.vanderbiltchemicals.com
David Como Molykote P.O. Box 0994 Midland, MI 48686
Joe Kaperick Afton Chemical Corporation 500 Spring St. Richmond, VA 23218-2158
Jim Hunt Tiarco Chemical 1300 Tiarco Drive Dalton, GA 30720
Dr. Anoop Kumar Royal Manufacturing Co., LP 516 S, 25th West Ave. Tulsa, Oklahoma 74127
Chuck Coe Grease Technology Solutions LLC 35386 Greyfriar Dr Round Hill, VA 20141
Crystal O’Halloran, MBA, CAE NLGI International Headquarters 249 SW Noel, Suite 249 Lee’s Summit, MO 64063
Serving the Grease Industry Since 1933 – VOL. 82, NO. 1, MARCH/APRIL 2018
4 President’s Podium STRATCO Contactor Reactor and Its Use In the 6 The Production of Calcium Sulfonate Based Greases ®
DIRECTORS Barbara Bellanti Battenfeld Grease & Oil Corp. of NY P.O. Box 728 • 1174 Erie Ave. N. Tonawanda, NY 14120 Richard Burkhalter Covenant Engineering Services 140 Corporate Place Branson, MO 65616 Willie Carter Calumet Branded Products, LLC One Purple Lane Porter, TX 77365 Maureen Hunter King Industries, Inc. Science Road Norwalk, CT 06852 Gian L. Fagan Chevron Lubricants 100 Chevron Way Room 71-7338 Richmond, CA 94802 Tyler Jark Lubricating Specialties Co. 8015 Paramount Blvd. Pico Rivera, CA 90660 Timothy Langlais Ergon, Inc. P.O. Box 1639 Jackson, MS 39215 Wayne Mackwood Lanxess Corporation 565 Coronation Dr West Hill, Ontario, M1E 2K3 Canada Matthew McGinnis Daubert Chemical Company 4700 S. Central Ave. Chicago, IL 60638
Dwaine (Greg) Morris Shell Lubricants 526 S. Johnson Drive Odessa, MO 64076 George Sander FMC Corporation 2801 Yorkmont Rd., Suite 300 Charlotte, NC 28208 John Sander Lubrication Engineers, Inc. P.O. Box 16447 Wichita, KS 67216 Tom Schroeder Axel Americas, LLC P.O. Box 12337 Kansas City, MO 64116 Simona Shafto Koehler Instrument Co. 85 Corporate Dr. Holtsville, NY 11716 Thomas W. Steib The Elco Corporation 1000 Belt Line Street Cleveland, OH 44109 Pat Walsh Texas Refinery Corp. One Refinery Place Ft. Worth, TX 76101 Mike Washington The Lubrizol Corporation 29400 Lakeland Blvd. Mail Drop 051E Wickliffe, OH 44092 Ruiming “Ray” Zhang R.T. Vanderbilt Company, Inc. 30 Winfield St. Norwalk, CT 06855
TECHNICAL COMMITTEE CO-CHAIRS:
CHAIR, SESSION PLANNING:
Chad Chichester Molykote 2200 W. Salzburg Rd., C40C00 Midland, MI 48686
Wayne Mackwood Lanxess Corporation 565 Coronation Dr West Hill, Ontario, M1E 2K3 Canada
David Turner CITGO 1293 Eldridge Parkway Houston, TX 77077
EDITORIAL REVIEW COMMITTEE CHAIR:
Joe Kaperick Afton Chemical Corporation 500 Spring St. Richmond, VA 23218-2158
Mary Moon, PhD, MBA Presque Isle Innovations LLC 47 Rickert Drive Yardley, PA 19067
John J. Lorimor, Axel Americas, LLC. & John S. Kay, STRATCO Inc.
Calcium Sulfonate-Based Grease 14 Application Technologies:of New From Laboratory to Field J. Andrew Waynick, NCH Corporation
Typical Application of Calcium Sulfonate Complex Greases 32 The in Steel Mills Li Jiwei, Cheng Shutian, Zhao Wei, Wu Baojie, Tianjin Branch, SINOPEC Lubricant CO., LTD.
Grease Microstructure 40 Novel and itsPolymer Proposed Lubrication Mechanism S. Chatra, D. Muller, C. Matta, R. Thijssen, M. N. bin Yusof and M. C. P. van Eijk , SKF Engineering & Research Centre
Grease Thickeners: How to Navigate your Way 50 Lubricating through the Lithium Crisis Gareth Fish, PhD CLS CLGS, Chris Hsu, PhD, and Robert Dura, PhD The Lubrizol Corporation
62 2018 Calendar of Events 65 A dvertiser’s Index ON THE COVER
Application of New Calcium Sulfonate-Based Grease Technologies: From Laboratory to Field Page 14
Published bi-monthly by NLGI. (ISSN 0027-6782) CRYSTAL O’HALLORAN, Editor NLGI International Headquarters 249 SW Noel, Suite 249, Lee’s Summit, MO 64063 USA Phone (816) 524-2500, FAX: (816) 524-2504 Web site: http://www.nlgi.org - E-mail: email@example.com The NLGI Spokesman is a complimentary publication. Past issues may be found on the NLGI Website, www.nlgi.org The NLGI Spokesman is indexed by INIST for the PASCAL database, plus by Engineering Index and Chemical Abstracts Service. Microfilm copies are available through University Microfilms, Ann Arbor, MI. The NLGI assumes no responsibility for the statements and opinions advanced by contributors to its publications. Views expressed in the editorials are those of the editors and do not n ecessarily represent the official position of NLGI. Copyright 2017, NLGI. Postmaster: Send address corrections to the above address.
IMPORTANT NOTE: The CLGS exam will be given at the 2018 NLGI Annual Meeting on Tuesday, June 12th at 10AM. Please contact firstname.lastname@example.org to enroll in this course.
John Sander, Chair In the world of maintenance and lubrication, several lubricant-related technical organizations now certify lubrication expertise. These include the International Council for Machinery Lubrication (ICML), the Society of Tribologists & Lubrication Engineers (STLE), and NLGI International. Each has an established program that documents the major criteria for demonstrating knowledge and skill in lubricants and lubrication practices. But only NLGI’s Certified Lubrication Grease Specialist program identifies those individuals who have true expertise in lubricating grease. The letters CLGS after one’s name signify both fundamental and extended knowledge of grease formulations, grease processing, grease testing and grease applications.
and having the letters “CLGS” on one’s business card sends a message the others don’t: It says the individual possesses a defined level of expertise that is specific to the field of grease, and that NLGI recognizes this achievement.
This is important because grease doesn’t behave like other lubricants. It typically is produced in a sophisticated reaction process (not simply blended like other lubricants), and it requires unique understanding to correctly formulate, test, select and apply. While the other programs focus primarily on fluid lubrication but include some lubricating grease fundamentals, the NLGI’s Certified Lubricating Grease Specialist program deals almost exclusively with lubricating grease.
Obtaining CLGS begins with a closely monitored twohour written examination. An 80 percent or better score is required for successful certification, which extends for a three-year period. To maintain certification, the candidate must renew their certification every three years and submit documentation to NLGI of continuing professional development, such as:
As a member of the NLGI Board of Directors, I know this first-hand. I hold credentials from all three of the groups,
Certification entitles one to use the copyrighted CLGS designation, and to be listed on the NLGI website as a grease expert. It can be a professional advantage in obtaining employment or going after business opportunities that require grease expertise, and it brings immediate credibility when working with customers. Employers use CLGS certification to screen potential employees, and OEMs and end users can use it to ensure that their suppliers are qualified to make grease recommendations.
• Attend an NLGI annual meeting • Present a paper at an NLGI annual meeting
-4VOLUME 82, NUMBER 1
Is inadequate product testing putting your company at risk? We made the
Product Improvement Test Results
Increased Sales Report 2017
Don’t wait to find out . . . Our experience with over 600 standard, industry, and customized test methods enables us to offer the best assurance of product quality. We work closely with you to target product end use conditions with a selection of the most appropriate tests.
Petro-Lubricant Testing Laboratories, Inc. A uniquely independent analytical tribology testing company… …with hundreds of clients around the world and a staff of scientists experienced with an extensive range of product types and applications.
ISO 9001 and ISO/IEC 17025 certifications email@example.com www.petrolube.com Lafayette, NJ 07848 973-579-3448
-5NLGI SPOKESMAN, MARCH/APRIL 2018
The STRATCO® Contactor™ Reactor and Its Use In the Production of Calcium Sulfonate Based Greases By: John J. Lorimor, Axel Americas, LLC. & John S. Kay, STRATCO Inc.
water. Unlike other grease types, these excellent performance characteristics are present in the grease without the use of additional compounding or additives1.
Calcium sulfonate based greases are recognized as an excellent technology for grease applications where heat, water, and high or shock loads exist. Their inherent Figure 1. Calcium sulfonate type grease global production volumes properties are well known and include excellent rust and wear protection, high load carrying capacity, high dropping point, and excellent mechanical stability, even in the presence of water. Calcium sulfonate based greases are typically prepared in conventional “open” kettles. The design of this type of production vessel is limited in its mixing and heating effectiveness. The unsealed construction of these kettles allows the volatile promoters used in the calcium sulfonate grease production process to escape. In addition, the slow speed mixing imparted by paddle stirring is not optimal for production of a dispersed micelle structure. In contrast, the STRATCO® Contactor™ reactor was designed to address the limitations of Calcium sulfonate based greases are used frequently as conventional open kettles for reacting grease thickeners. The problem solvers in severe service applications where other STRATCO Contactor reactor’s sealed design, highly efficient greases have failed because they could not survive the rate of heat transfer, turbulent circulation path, and high shear extreme conditions. Some of the demanding applications mixing zone make it extremely well suited as a production that have benefitted from calcium sulfonate type greases are vessel for calcium sulfonate based greases. found in steel, pulp and paper mills, off-road construction The objective of this project is to successfully manufacture and mining equipment, marine, and even food processing calcium sulfonate based greases using the STRATCO industries. As shown in Figure 1, the direct result of this Contactor reactor. The differences in manufacturing processes successful performance is that calcium sulfonate based for conventional open kettles and the STRATCO Contactor greases have become one of the fastest growing types of grease reactor will be discussed in detail. Performance characteristics globally2. Because of this popularity and high growth rate, of the finished calcium sulfonate based greases obtained by grease producers are increasingly looking to produce calcium each process will be compared. sulfonate based greases.
Calcium sulfonate based greases excel in demanding lubricant applications where machinery is exposed to heat, water, and high or shock loads. These highly shear stable greases provide excellent protection against rust and wear in these extreme environments, even in the presence of
The earliest type of calcium sulfonate based grease is commonly referred to as a calcium sulfonate gel or “simple” calcium sulfonate grease. In this most basic version, the thickener component of the grease comprises only a gelled
-6VOLUME 82, NUMBER 1
overbased calcium sulfonate. The overbased precursor for this grease contains a large proportion of non-crystalline calcium carbonate dispersed within a sulfonate matrix. During production, suitable promoters such as water, alcohols, and acids are added to the mixture of calcium carbonate and sulfonate materials, followed by heating within the proper temperature range, to convert this amorphous calcium carbonate into its crystalline form (calcite). This crystallization causes the rheology of the mixture to change from a liquid into a viscous or semi-solid gel. At this point, the mixture still contains water and must be dehydrated and adjusted with additional oil to produce a lubricating grease. For the production of a calcium sulfonate complex grease, additional reactions take place after the basic carbonate conversion step to produce a secondary thickener that is compatible with calcite. The secondary soap/salt complex ingredients are typically comprised of 12-hydroxystearic acid and a complexing acid such as boric or acetic, reacted with calcium hydroxide. As with the simple sulfonate greases, water must be removed since it is used as a conversion promoter. In addition, water is also produced during secondary thickener soap forming reactions.
and recirculated to help turn the product over and encourage better mixing. Volatile promoters used in the calcium sulfonate grease production process can escape from these open kettles into the atmosphere. This causes the grease to form with reduced structure and soft consistency. In addition, the slow speed mixing imparted by paddle stirring is not optimal for production of a dispersed micelle structure.
STRATCO Contactor reactor
The STRATCO Contactor reactor (as shown in Figure 3) consists of a pressure vessel, a circulation tube, and a hydraulic head assembly complete with the mixing impeller and driver. The STRATCO Contactor reactor, by design, has a highly turbulent circulation path. All energy input through the mixing impeller is expended within the materials being mixed. The high dispersion mixing in the STRATCO Contactor reactor is achieved by the proprietary hydraulic head assembly. Frequent and forced changes in velocity and direction of flow occur around the impeller area. This results in a zone of high shear and intense mixing, which reduces the time required to complete the saponification reaction. Figure 3. STRATCO Contactor Reactor
Calcium sulfonate based greases are typically produced in conventional â€œopenâ€? kettles, so called for their operation under atmospheric pressure. This type of production vessel (as shown in Figure 2) is limited by the basic design in its Figure 2. Conventional atmospheric kettle
mixing and heating effectiveness, typically utilizing paddles for stirring and an external jacket for heat transfer fluid. The agitation, which may be counter rotating, is typically operated at speeds below 20 rpm. The kettle contents may be pumped
Figure 4 shows the flow through the STRATCO Contactor. Material is pulled down through the center of the circulation tube by the impeller, reversed, and then forced up through the annular space. Because the impeller is located on the bottom, dry materials are kept in suspension until they dissolve or react. The heating medium is circulated through the double-walled circulation tube inside the STRATCO Contactor. The outside
-7NLGI SPOKESMAN, MARCH/APRIL 2018
Figure 4 - Flow through the STRATCO Contactor
liter) conventional open finishing kettle. An electric thermal heater and pump supplied heat transfer fluid for product heating up to a top temperature of 275°F (135°C). An air compressor was used to pressurize the contactor during low temperature steps to 50 psi (107 hPa). The equipment configuration is shown in Figure 5. The addition of a viewing port to the contactor reactor lid (as shown in Figure 6) allows the grease flow to be observed during pressurized operation (as shown in Figure 7). Monitoring and maintaining grease flow is important, as calcium sulfonate type greases can become very thick during the production process. In this project, maintaining proper flow and mixing of the experimental greases required using the full base oil requirement of the formula during the reaction stage. No oil would was used in the finishing stage. Figure 5. STRATCO Pilot Plant
of the STRATCO Contactor reactor is also jacketed. Because of the double-walled circulation tube and the outside jacket on the shell, the STRATCO Contactor reactor has approximately three times the heat transfer area of an open kettle type reactor of the same volume. The flow path forces the circulating material to remain in contact with the total heating surface area at all times. Also, the heat transfer in the STRATCO Contactor reactor is enhanced by the high velocity of material flowing past the heat transfer surfaces. Figure 7. View of grease For the production of calcium sulfonate type grease, Figure 6. Viewing port through viewing port there would appear to be several advantages to the use of a STRATCO Contactor reactor instead of the conventional open kettle. Since the STRATCO Contactor is a sealed design, there would be no loss of volatile promoters from the mixture. The large heat transfer area would allow quick heating to reaction temperatures. The turbulent circulation path and high shear mixing zone would cause more intense mixing, and could improve micelle dispersion. The operation of the unit under pressure may also be able to provide a faster and more complete conversion of the amorphous calcium carbonate into its crystalline form. Therefore, the objective of this project is to successfully manufacture calcium sulfonate based greases using the STRATCO Contactor, and understand if any of these equipment differences offer any advantages in the production Techniques for conversion of overbased calcium sulfonates of calcium sulfonate type greases when compared to the use of into multi-purpose lubricating greases are well detailed in the conventional open kettle manufacturing methods. literature3. For the production of the experimental greases in this study, two different sulfonate conversion methods Experimental from the literature were attempted. The first approach used a Equipment used in the study included a 6-gallon (22 liter) commercially sourced proprietary overbased calcium sulfonate STRATCO Contactor pilot plant reactor and 10-gallon (38 “pre-mix” designed for easy grease production. In addition to -8VOLUME 82, NUMBER 1
the overbased calcium sulfonate, the mixture also contained a proprietary conversion promoter system. This production method only required the addition of base oil and water to complete the grease recipe. The second conversion approach was more conventional, where the grease was made entirely from individual components, including promoters. Two types of calcium sulfonate based greases were prepared. The first experimental grease was a “simple” calcium sulfonate grease. This type of grease is based upon the converted calcium sulfonate only, and does not contain any soap forming ingredients. In this system, the grease consistency is based entirely upon the thickening effect of the converted sulfonate. The second and third experimental greases were calcium sulfonate complex greases. Experimental grease 2 used the same initial ingredients and gelation procedure as grease 1, but then a secondary soap based thickener was formed in a separate saponification reaction step. Experimental grease 3 used a full component based approach for the production of a calcium sulfonate complex grease. In all cases, the specific formulations were designed to achieve NLGI grade 2 consistency.
Experiment 1: Calcium sulfonate gel
Experiment 2: Calcium sulfonate complex A
Experiment 3: Calcium sulfonate complex B
Formulation ingredients: • Sulfonate pre-mix • 600N Group I base oil • Water
Formulation ingredients: • Sulfonate pre-mix • 600N Group I base oil • Water • 12-hydroxystearic acid • Acetic acid • Calcium hydroxide
Formulation ingredients: • 400 TBN Ca sulfonate • High boiling glycol • Sulfonic acid • Water • 600N Group I base oil • 12-hydroxystearic acid • Acetic acid • Calcium hydroxide
Manufacturing procedure: 1. Mix sulfonate, oil, and water 2. Pressurize STRATCO Contactor to 50 psi (107 hPa) 3. Heat at 193°F (89°C) until conversion to calcite occurs 4. Product is dehydrated by heating to 250-300°F (121-149°C) and transferred to finishing kettle
Manufacturing procedure: 1. M ix sulfonate, oil, and water 2. P ressurize STRATCO Contactor to 50 psi (107 hPa) 3. H eat at 193°F (89°C) until the conversion to calcite occurs 4. O nce gelled, depressurize and add soap forming ingredients, repressurize to 50 psi (107 hPa) 5. H old at 190-200°F (88°C-93°C) to complete saponification 6. P roduct is dehydrated by heating to 250-300°F (121-149°C) and transferred to finishing kettle
Manufacturing procedure: 1. Mix sulfonate, oil, promoters, and water 2. Pressurize STRATCO Contactor to 50 psi 3. Heat at 193°F (89°C) until the conversion to calcite occurs 4. Once gelled, depressurize and add soap forming ingredients, repressurize to 50 psi 5. Hold at 190-200°F (88°C-93°C) to complete saponification 6. Product is dehydrated by heating to 250-300°F (121-149°C) and transferred to finishing kettle
The grease was sampled from the STRATCO Contactor at various intervals during the pressurized conversion step in order to determine the actual time to convert the amorphous calcium carbonate into its crystalline calcite form. These samples were kept and analyzed after the production had taken place. As shown in Figure 8, upon checking the samples by FT-IR for conversion, it was found that the actual conversion had taken place within the first 30 minutes of the 3-hour hold time in the Contactor. This represents a significant change from conventional open kettle manufacturing, where the conversion time can take anywhere from 3 to 6 hours. As such, it was determined that an optimized process would only require a 30-minute conversion step.
-9NLGI SPOKESMAN, MARCH/APRIL 2018
Figure 8. FT-IR spectra comparison of gelation time
Manufacturing process comparison
The manufacturing process steps and timing between conventional open kettle and optimized STRATCO Contactor process were recorded in Figure 9. The red color blocks indicate events occurring in the heated vessel, and the blue color blocks indicate those events occurring in the cooling vessel. As shown, the conventional open kettle cooking process can produce a single batch of calcium sulfonate complex grease over two standard 8-hour shifts. By comparison with an optimized STRATCO Contactor reactor cooking process, the shorter process cycle time could allow the production of up to two batches of calcium sulfonate complex grease during the same two 8-hour shifts.
- 10 VOLUME 82, NUMBER 1
Figure 9. Manufacturing process comparison
- 11 NLGI SPOKESMAN, MARCH/APRIL 2018
Comparison of finished grease properties
As previously reported, the experimental grease formulations made in the Contactor were identical to those expected to achieve NLGI grade 2 consistency at 100% yield in an open kettle process. In the case of experimental greases 1 and 2 based upon the sulfonate pre-mix, this was exactly what was obtained. However, in the production of experimental grease 3 using the component approach, the grease at 100% yield unexpectedly had the consistency of NLGI grade 4 grease. Grease 3 would require an extra oil addition of 20% by weight to reach NLGI 2 consistency.
Figure 10. Experimental greases obtained from STRATCO Contactor process
Once all greases were at the same relative consistency, the performance characteristics of the finished calcium sulfonate based greases obtained by each process were compared by standardized ASTM test methods. The results are shown in Table 1. Based upon experience, the performance test results are similar to what would be expected from the same greases manufactured in a conventional open kettle process.
Table 1. Performance characteristics of the finished experimental greases
- 12 VOLUME 82, NUMBER 1
Conclusions drawn from the experimental work
The STRATCO Contactor reactor was designed to address the limitations of conventional grease cooking kettles. The STRATCO Contactor reactorâ€™s sealed design, highly efficient rate of heat transfer, turbulent circulation path, and high shear mixing zone make it extremely well suited as a production vessel for calcium sulfonate based greases. Conversion of the amorphous calcium carbonate into calcite was observed to be faster in the Contactor process than in typical conventional open kettles. In one case, an improvement in grease yield over the conventional process was observed. The resulting greases obtained from the STRATCO Contactor process were demonstrated to have similar overall performance to the greases obtained from more conventional manufacturing equipment. For the full-scale manufacturing plant, these experiments have shown that the use of the STRATCO Contactor has potential to improve process speed in the production of calcium sulfonate type greases. Faster production may improve equipment utilization, labor efficiency, and energy consumption. With a shorter process cycle, there is clear potential for increasing manufacturing output by producing more batches in the same period of time.
The authors wish to acknowledge Nathan Claycamp of AXEL Americas, LLC for his contribution in the performance testing of the finished greases.
1. M ackwood, W. and Muir, R., Calcium Sulfonate Greasesâ€Ś One Decade Later, NLGI Spokesman, Vol 63, No 5, pp 24-37, 1998. 2. G rease production survey reports for the calendar years 2009-2015, NLGI 3. D enis, R., Sivik, M., Calcium Sulfonate Grease-Making Processes, Presented at 75th Annual NLGI Meeting, June 7, 2008, Williamsburg, Virginia
- 13 NLGI SPOKESMAN, MARCH/APRIL 2018
Application of New Calcium SulfonateBased Grease Technologies: From Laboratory to Field By: J. Andrew Waynick, NCH Corporation ABSTRACT
Calcium sulfonate-based greases were first developed in the 1960â€™s, and multiple improvements and refinements have been made since then. Recently, two modifications of this class of lubricating grease have been developed: adding powdered calcium carbonate or powdered calcium hydroxyapatite as the sole calcium-containing base for reaction with complexing acids, and adding this material pre-conversion. The chemistry, composition, and manufacturing aspects of these two modifications were evaluated against four technical assertions found in the prior calcium sulfonate grease literature. Results showed that only two of those prior technical assertions are still valid for these two new calcium sulfonate grease modifications. Based on the relative merits and limitations apparent from that laboratory work, final formulations were developed for two specific applications: open gear drives and braided wire rope lubrication. Initial field results are provided, and conclusions are discussed.
The first calcium sulfonate-based greases can actually trace their beginnings to the development of the highly overbased calcium alkyl benzene sulfonates from which they are made. As that overbased calcium sulfonate technology continued to advance, the first calcium sulfonate-based greases were eventually invented2. Those first greases were simple calcium sulfonate thickened products that were primarily used as rust preventative coatings1. Nearly 20 years later, in the 1980â€™s calcium sulfonate complex greases were first documented as a way to reduce the required level of the overbased calcium sulfonate, improve the low temperature mobility, and make the final products more suitable for a wider range of applications. Since that time, several additional modifications (process and composition) of the original calcium sulfonate complex grease chemistry
have been developed4,5,6. These developments have already been reviewed several times7,8 and will not be elaborated upon here. Instead, four important literature assertions from the first simple and complex calcium sulfonate grease development are summarized so as to provide a proper setting for the experimental work described within this paper. Those four prior literature assertions are: 1. Successful conversion of the overbased calcium sulfonate to an initial grease structure will not occur in the presence of basic calcium-containing solids not part of the overbasing structure. 2. Maximum dropping point of the final grease requires that all water be removed as promptly as possible after conversion is complete. 3. Added calcium carbonate is not a suitable calciumcontaining base for reaction with complexing acids. Only calcium oxide or calcium hydroxide as exclusively mentioned in the prior literature are suitable for this purpose. 4. Thickener yield can be improved when all or a part of the complexing acids are added pre-conversion instead of only post-conversion (as was required in the first documented calcium sulfonate complex greases). These four prior literature assertions are discussed as follows. The first prior literature assertion involves the effect of calcium-containing bases not part of the overbased calcium sulfonate on the initial conversion process whereby a calcium sulfonate grease is made. Simple calcium sulfonate greases were first documented in a series of U.S. Patents2,9,10,11,12. These patents described the process whereby an overbased calcium alkyl benzene sulfonate was first formed by controlled
- 14 VOLUME 82, NUMBER 1
reaction of calcium oxide and/or calcium hydroxide with an alkyl benzene sulfonic acid, water, one or more promoters, and carbon dioxide. When properly carried out, this process (promotion) resulted in a large stoichiometric excess of calcium carbonate incorporated into a non-crystalline (“amorphous”) form within the sulfonate. This overbased calcium sulfonate was then reacted with water and one or more non-aqueous converting agents to form a grease-like structure (conversion). The detailed chemical mechanisms of both the promotion and conversion processes have never been disclosed in the open literature. However, the first simple calcium sulfonate patents did teach that for the conversion process to be successful, excess unreacted calcium-containing material (not part of the overbased structure) needed to first be removed from the overbased calcium sulfonate. This was accomplished by filtering the previously formed overbased calcium sulfonate to remove non-colloidal dispersed solid basic material2,9,10,11. In fact, every one of the numerous examples in these first simple calcium sulfonate grease patents described the filtration of the overbased calcium sulfonate as the process step immediately prior to attempting conversion. Based on the previous patent literature covering the formation of overbased calcium sulfonates1, this basic material (removed by filtration) would include unreacted calcium oxide/hydroxide as well as any calcium carbonate that had formed during the promotion process but had not been incorporated within the amorphous structure. Eventually, this restriction was softened by claiming that if the solid basic material was not removed prior to conversion, a grease structure could form. However, the grease would not be as uniform and firm (reduced thickener yield)12 as what would result if the basic material had been removed before conversion This restriction was implicitly restated almost 30 years later in a U.S. Patent describing a thickener yield improvement in calcium sulfonate complex greases. In that patent5, several methods to improve thickener yield were provided whereby some of the complexing acids were added pre-conversion as well as post-conversion. Although one such method also allowed for the pre-conversion addition of calcium hydroxide, such addition was taught to be less desirable in terms of its impact on thickener yield. Additionally, none of the claims included pre-conversion addition of calcium hydroxide. There is no reason to believe that the necessity of preconversion removal of calcium-containing solids was incorrect at the time it was first taught in the 1960’s. However, overbased calcium sulfonates are not entirely the same today compared to 50 years ago. The overbased calcium sulfonates typically described in those 1960’s patent examples were produced from the sulfonation of petroleum fractions, i.e. petroleum
or natural sulfonic acids13,14,15,16. Similarly, the examples from the first simple calcium sulfonate grease patents (as previously cited) also used petroleum-derived sulfonates. Also, it had been taught that as much as 25% of the calcium oxide/hydroxide present in the final overbased calcium sulfonate could remain non-carbonated, i.e. incorporated into the overbased structure, but remaining as the oxide and/or hydroxide form2. In contrast, much of today’s overbased calcium sulfonates derive entirely or in part from synthetic alkylated sulfonic acids wherein the number of alkyl groups, the chain length, and the degree of branching are different. Also, the amount of non-promoted calcium oxide/hydroxide is typically much lower. For instance, some of today’s overbased calcium sulfonates have Strong Base Number (SBN) values at or below 30 mg KOH/g. Since the Total Base Number (TBN) of these overbased sulfonates are typically 400 mg KOH/g, the amount of non-promoted calcium base in such products can be 7.5% or even lower. Since it has been recently shown that the SBN value of the overbased calcium sulfonate can affect the conversion process whereby calcium sulfonate-based greases are formed17, it stands to reason that restrictions placed on the conversion process 50 years ago may no longer apply as when they were first stated. The second prior literature assertion describes a potential harmful effect on simple calcium sulfonate greases caused by the water used during the conversion process. More specifically, one early U.S. Patent taught that the water required for the conversion process should be removed as soon as possible after conversion was achieved. Failure to do so would result in reduced thickener yield and dropping point18, with dropping point being the property most adversely affected. Other than the data provided in this patent, there appears to be little additional work to substantiate or refute this claim. Interestingly, nearly all the calcium sulfonate complex grease technologies that were subsequently published in U.S. Patents taught the post-conversion addition of boric acid in water with the water removed later in the process as the grease was heated to its top temperature. As already mentioned, all of this work was done decades ago when the detailed composition of overbased calcium sulfonates may have been different from what is often used today. The third prior literature assertion describes an adverse effect associated with the presence of calcium carbonate when attempting to form calcium sulfonate or calcium soapthickened greases. A 1974 U.S. Patent covered a one-step process of making a simple calcium sulfonate grease from calcium hydroxide, alkyl benzene sulfonic acid, water, a promoter/converter, and carbon dioxide. This patent stated that the calcium hydroxide must contain no more than 5%
- 15 NLGI SPOKESMAN, MARCH/APRIL 2018
calcium carbonate in order for the process to be successful19. Since sulfonic acids are much stronger acids than carboxylic acids, this assertion implies that calcium carbonate may not be a good choice for reaction with typical complexing acids used in calcium sulfonate complex greases. Similarly, the first calcium sulfonate complex grease patent taught that the added calcium hydroxide used for reaction with complexing acids must be 96% to 98% pure and free of impurities3. It is well known that the primary impurity present in calcium hydroxide is calcium carbonate formed by slow reaction with carbon dioxide in air20. Also, Bonerâ€™s often-used grease reference book (1954 edition) documented the harmful effect of calcium carbonate as an impurity in calcium hydroxide used to make calcium soap greases. All these teachings from the established literature indicate that calcium carbonate should not be used as the sole added base for reaction with complexing acids when making calcium sulfonate complex greases. However, overbased calcium sulfonate chemistry has significantly changed since those prior literature assertions were first published. The fourth prior literature assertion involves the addition of complexing acids either before or both before and after conversion as a method to improve thickener yield5,6 of calcium sulfonate complex greases. This is in contrast to the first documented calcium sulfonate complex grease where complexing acids were only added after conversion3. The next section describes how those four prior literature assertions were re-evaluated in this study.
EXPERIMENTAL General Approach Two new calcium sulfonate-based grease chemistry modifications have been developed recently17. These two new chemistry modifications are as follows: 1. Using added (powdered) calcium carbonate as the sole calcium-containing base for reaction with complexing acids, and adding this material pre-conversion. 2. Using added (powdered) calcium hydroxyapatite as a calcium containing base for reaction with complexing acids, and adding this material pre-conversion. A complete reporting of this development work for these two chemistry modifications would be well outside the scope of this paper due to the sheer number of laboratory grease batches prepared. However, a representative selection taken from that work was chosen to illustrate some of the more
important aspects of the two chemistry modifications. Specifically, the laboratory work documented in this paper was chosen to re-evaluate the four prior literature assertions discussed in the previous section, and to determine if those assertions still applied to the two new calcium sulfonate-based grease chemistry modifications. This was done by examining the two chemistry modifications in light of the corresponding four effects: 1. The effect of the pre-conversion presence of some calciumcontaining bases on the conversion process as indicated by the resulting calcium sulfonate-based greases (relating to the first prior literature assertion). 2. The effectiveness of using calcium-containing bases other than calcium oxide/hydroxide for reaction with complexing acids (relating to the third prior literature assertion). 3. The effect of water on the conversion process and resulting grease properties (relating to the second prior literature assertion). 4. The effectiveness of splitting the addition of complexing acids before and after conversion as a method to improve thickener yield (relating to the fourth prior literature assertion). Consequently, each of the two chemistry modifications was used to develop a formulation selected for one of two targeted commercial applications: open gear lubrication and braided wire rope lubrication. The criteria for the selection process were based on various performance requirements of the two applications and how those performance requirements matched up with the performance properties of the two chemistry modifications. Actual results from early commercial field trials are reported as well. Conclusions are then provided as supported by the results. Equipment, Test Methods, and Raw Materials All greases were made using a Kitchen Aid-style mixer with a planetary stirrer and heating mantle. All weights were measured using an open pan analytical balance capable of measuring to the nearest 0.01 g. Each grease was given three passes through a three-roll mill with both gaps set at 0.001 inches (0.03 mm). Test methods used to evaluate the greases were dropping point by ASTM D2265 and penetration by ASTM D217
- 16 VOLUME 82, NUMBER 1
or D1403. A modified ASTM D2265 procedure was used wherein the block temperature was set at 343 C (650 F). This allowed each grease to experience the same thermal stressing during the test. It should also be noted that ASTM D2265 defines dropping points to values up to 316 C, and the correlation between ASTM D2265 values and real world grease performance is not defined at any temperature. However, since the modified dropping point method employed herein is used as a tool for detecting changes in grease structural stability, these concerns do not apply as long as the dropping point method used is consistently applied to all greases, and results are interpreted within the intended limitations of the investigation. The overbased calcium sulfonates used in this work had TBN values of about 400 mg KOH/g. The SBN values varied depending on the overbased calcium sulfonate used and are provided below as required. These values were determined by the suppliers. All TBN values were determined by ASTM D4739. SBN values were determined by a proprietary method that provides the same results as ASTM D4739, but with greater precision. The units of mg KOH/g for TBN and SBN will be understood to apply to all TBN and SBN values throughout this paper without actually using those units within the text. Kinematic viscosities were determined by ASTM D445. Other test methods used in this work are cited as required. All raw materials were essentially 100% pure unless otherwise indicated. Calcium hydroxide, calcium carbonate, anhydrous calcium sulfate, and calcium hydroxyapatite were all food grade purity with a mean particle size below 5 microns.
RESULTS AND DISCUSSION Chemistry Modification No. 1 A series of four calcium sulfonate greases was made with the same final composition based on the unreacted percentages of components. The overbased calcium sulfonate used was a synthetic-derived product with an SBN value that was about 40. This sulfonate will be referred to as overbased calcium sulfonate A1 in this paper. In these greases as well as all the others discussed in this paper, conversion was achieved by the addition of an alkylene glycol and water. The water was added at 4.5% based on the total weight of all components prior to any chemical reactions. However, water is not included in any of the formulations of this paper since it is not present in final greases due to process heating. Conversion was also assisted by the addition of a small amount of essentially dodecyl benzene sulfonic acid (DDBSA), as is commonly used in the preparation of calcium sulfonate-based greases. The DDBSA was added to the initial portion of base oils and the overbased calcium sulfonate A. The resulting blend was allowed to mix for 20 minutes before proceeding to the next step. This was done for all the greases described in this paper. Powdered calcium carbonate was added either before or after conversion as the calcium-containing base for reaction with complexing acids. The complexing acids used for these first four greases were 12-hydroxystearic acid (12-HSA), acetic acid, and phosphoric acid. The formulation for these four greases (Greases 1 â€“ 4) is provided below in Table 1.
Finally, appropriate safety measures were used during the preparation and testing of all greases in this paper.
- 17 NLGI SPOKESMAN, MARCH/APRIL 2018
The general process profile for making these four greases is provided below in Figure 1.
Although Figure 1 provides a general profile for how Greases 1 â€“ 4 were made, there were process differences. Those differences along with penetration and dropping point data are provided below in Table 2. Several important observations can be made. First, note that the only difference between Greases 1 and 2 was when the calcium carbonate was added relative to conversion. By comparing these two greases, it is apparent that adding calcium carbonate before conversion improved the thickener yield and dropping point compared to adding the same amount of calcium carbonate after conversion. Adding calcium carbonate as a basic calcium-containing material before conversion does not appear to hinder the conversion process, at least when using this particular overbased calcium sulfonate. Thus, the first prior literature assertion (concerning the adverse effect of calcium-containing bases present during conversion) does not apply to this formulation under these conditions. A second observation relates to the use of added calcium carbonate as an effective calcium-containing base for reaction with complexing acids. This can be seen by looking at Greases 3 and 4 compared to Grease 1. When no calcium carbonate was added (Grease 3), the first two complexing acids added pre-conversion reacted with the small amount of internal calcium hydroxide derived from the overbased calcium sulfonate. Since that amount of calcium hydroxide was not sufficient to react with all the complexing acids, the only other source of basic calcium, a portion of the amorphous calcium carbonate derived from the overbased calcium sulfonate, had
to react. This reduced the amount of amorphous calcium carbonate left to form the initial simple calcium sulfonate grease structure. Although Fourier Transform Infrared Spectroscopy (FTIR) showed that the remaining amorphous calcium carbonate changed to crystalline calcium carbonate during conversion process of Grease 3, no significant grease structure formed. It has already been established that if there is not enough amorphous calcium carbonate in the overbased sulfonate, a distinct grease structure may not form upon conversion2. On the other hand, when the complexing acids were added after the initial simple calcium sulfonate grease had formed but before the post-conversion addition of the calcium carbonate (Grease 4), the complexing acids were forced to react with the calcium-containing bases derived from the overbased calcium sulfonate. This resulted in a thickener yield lower than Grease 1 or 2 where added calcium carbonate was present and available for reaction. These data indicate that added calcium carbonate can be an effective calcium-containing base for reaction with complexing acids when making calcium sulfonate complex greases, at least when using this particular overbased calcium sulfonate. Thus, the third prior literature assertion (stating that only added calcium oxide or calcium hydroxide are appropriate for reaction with complexing acids) does not apply to this formulation under these conditions. The effect of the concentration of water during conversion was evaluated by making three more greases exactly like
- 18 VOLUME 82, NUMBER 1
Grease 1 except for the amount of water added at the beginning of the process. These three greases (Greases 5 â€“ 7) had water concentrations ranging from 1.1% to 9.0%. The information and test data on these greases are provided below in Table 3. The information on Grease 1 is also included for ease of comparison.
As can be seen, the dropping point was not significantly affected when the water concentration in the initial unconverted mixture ranged from 2.2% to 9.0%. However, when the water concentration was only 1.1%, conversion to a grease structure did not occur, even when the conversion step was continued for several more hours. This is likely due to the fact that water is required for conversion. If the initial water concentration is too low, conversion does not occur. This effect is magnified when the conversion process is done under open conditions where the concentration of water decreases over time due to evaporation. At the other extreme, when 9.0% water was added, an apparent reduction in thickener yield occurred compared to the other three greases in Table 3. So adding too little water can result in no conversion; adding too much can result in loss of thickener yield. The effect of post-conversion prolonged presence of water on thickener yield and dropping point was evaluated by making three more greases (Greases 8 â€“ 10). These greases were also prepared exactly like the previous three greases except for one point: after conversion was complete, each grease was held for two hours before adding the complexing acids and heating to top temperature. Results are provided in Table 4. Once again, Grease 1 is included for ease of reference.
- 19 NLGI SPOKESMAN, MARCH/APRIL 2018
As can be seen, the prolonged post-conversion presence of water did not have much effect on thickener yield as evidenced by the small variation in worked penetration values in Greases 8 - 10. However, dropping point was adversely affected by the prolonged post-conversion presence of water. The greatest reduction in dropping point relative to Grease 1 was in Grease 8 where the highest level of water was initially present. All greases were prepared under open conditions, and the two hour delay after conversion was at 88 C (190 F). Under these conditions, a higher initial water concentration would translate to water being present at higher levels for longer periods of time. This is exactly the trend observed in the dropping points of Greases 8 â€“ 10 when compared to Grease 1. Thus, the second prior literature assertion (concerning the adverse effect of the prolonged post-conversion presence of water on final grease dropping point) appears to still be true when using this formulation approach and processing conditions.
Another five greases were prepared to evaluate the effect of adding a portion of the 12-HSA acid before conversion when making a grease similar to Grease 1. However, a different overbased calcium sulfonate was used in these greases compared to what was used in Greases 1 â€“ 10. This overbased calcium sulfonate B had an SBN value of about 60. Also, the extent of alkalization and the alkyl chain length were significantly different from the overbased calcium sulfonate A1 previously used. Grease 11A had all of its complexing acids added after conversion and was made according to the process profile of Figure 1. Greases 11B â€“ 14 were made according to the process profile provided in Figure 2. Final compositions and test data are provided in Table 5.
- 20 VOLUME 82, NUMBER 1
Greases 11A and 11B used 12-hydroxystearic, acetic, and phosphoric acids as complexing acids. Greases 12 – 14 used boric acid instead of acetic acid. The boric acid was added to 50 ml hot water, made into a slurry, and added to the grease after conversion, which was after the second portion of 12-HSA acid had been added, but before the phosphoric acid addition. It should be noted that the portion of the 12-HSA acid that was added before conversion was added at the beginning (after the initial base oil, PAO, DDBSA, and calcium carbonate had been added and mixed together at ambient temperature). As the initial mixture was heated to the conversion temperature (88 C), the 12-HSA acid would have melted (melting point is about 78 C) and dissolved in the base oil. Its reaction with basic components before this would be limited to how much was able to dissolve in the base oil prior to melting. This would likely be only a minimal amount given the large flaked appearance of 12-HSA acid. For Greases 11A and 11B, where the complexing acids were 12-HSA, acetic, and phosphoric acids, splitting the addition of the 12-HSA before and after conversion did not improve thickener yield and may have actually reduced it. For Greases 12 – 14, where the complexing acids included boric acid instead of acetic acid, there does appear to be some thickener yield improvement as the pre-conversion relative amount of 12-HSA is increased from 20% (Grease 12) to 100% (Grease 14). This is seen by recalculating the concentration of overbased sulfonate B in Greases 13 and 14 based on what those values would have been if additional base oil had been added so as to make their worked penetration value equal to 305 (the worked penetration value of Grease 12). This
calculation is done using an inverse linear relationship between the overbased sulfonate B concentration and the worked penetration. Those calculated values are provided in Table 5. They show that as the relative amount of pre-conversion 12-HSA is increased, thickener yield directionally increases. The dropping points for all four greases were excellent. Also, all four greases gave very high Four-Ball EP weld loads (620 to 800 kg). The thickener yield results are interesting based on prior literature results5,6. As already mentioned, previously reported work has shown that adding a portion of the 12-hydroxystearic acid before conversion can improve thickener yield (prior literature assertion 4). That previous work used boric acid but did not use phosphoric acid as a complexing acid. The only yield improving effect apparent in the Table 5 data involved the use of boric acid. However, the magnitude of yield improvement in Table 5 is not as large as previously reported. Possible reasons for this difference could include the use of phosphoric acid in Greases 12 – 14. Also, one must remember that the overbased calcium sulfonate B used in Greases 11A/B – 14 would be expected to be significantly different from what was likely used in that earlier work. This difference could be the reason for the differences between that earlier reported work and the results of Greases 11A/B – 14. However, it may also be due to the pre-conversion presence of added calcium carbonate. Data from Greases 1 – 4 have already shown that this added calcium carbonate is reacting with the complexing acids. The earlier cited literature work did not use calcium carbonate added preconversion. So, the presence of the added calcium carbonate
- 21 NLGI SPOKESMAN, MARCH/APRIL 2018
may have changed the reaction chemistry so as to modify the effect of pre-conversion 12-HSA on thickener yield. Further work would be needed to determine this with certainty. Thus, the fourth prior literature assertion (concerning thickener yield improvement when adding at least some of the complexing acids pre-conversion) appears to apply in varying degrees depending on the specific details of the formulations under these conditions. An additional observation can be made by comparing the composition and test data for Grease 11A (Table 5) with the composition and test data for Grease 1 (Tables 1 and 2). This observation concerns the relative thickener yield provided by overbased calcium sulfonates A1 and B. Grease 11A was made using the same process and complexing acids as Grease 1. The only difference between these two greases was the overbased calcium sulfonate used. Grease 1 had 36.0% overbased calcium sulfonate A1 (Table 1). Grease 11A had 29.95% overbased calcium sulfonate B. By comparing the worked penetrations of these two greases (Tables 2 and 5), it is apparent that overbased calcium sulfonate B gave a significantly better thickener yield compared to overbased calcium sulfonate A1 when all the complexing acids are added after conversion. Chemistry Modification No. 2 The second modification of previously established calcium sulfonate complex chemistry involved the use of calcium hydroxyapatite, Ca5(PO4)3OH, as a calcium-containing, hydroxide-providing base for reaction with complexing acids.
This approach was first disclosed two years ago21, and that work concentrated on chemical mechanistic details of calcium sulfonate complex reactions and their effect on dropping point. That work will not be repeated here. Instead, the focus of this work is similar to the above study of Chemistry Modification No. 1. Four greases, Greases 15 – 18, were made using calcium hydroxyapatite as the sole added base for reaction with complexing acids. The complexing acids were 12-HSA and acetic acid. Note that neither phosphoric nor boric acids were used. The overbased calcium sulfonate used for Greases 15 – 17 was the same sulfonate from the same supplier as the overbased calcium sulfonate A1 that was used in Greases 1 – 10. However, the overbased calcium sulfonate used for Greases 15 – 17 was from a different manufacturing lot. As a result, it had a somewhat lower SBN value of 35 compared to the SBN value of 40 that the overbased calcium sulfonate A1 had. Accordingly, the overbased calcium sulfonate used in Greases 15 – 17 will be referred to as overbased calcium sulfonate A2. Overbased calcium sulfonate B was used for Grease 18. The general process profile used to make Grease 15 is provided in Figure 3. The process profiles for Greases 16 – 18 were similar to Grease 15, but there were some differences. For Grease 16, the calcium hydroxyapatite was added after conversion but before the two complexing acids were added. For Grease 17,
- 22 VOLUME 82, NUMBER 1
the calcium hydroxyapatite was added at the beginning before conversion, and all of both complexing acids were added about 30 minutes thereafter. Grease 18 was exactly like Grease 17 except that overbased calcium sulfonate A2 was replaced with overbased calcium sulfonate B. Additionally, the total amount of hydroxide-equivalent base provided by the calcium hydroxyapatite and the internal calcium hydroxide in the overbased calcium sulfonate was calculated. The concentration of calcium hydroxyapatite was intentionally set at a level so that this total hydroxideequivalent basicity would be nearly twice what was required for complete reaction with all added acids (DDBSA and complexing acids). Final compositions and test data are provided in Table 6.
be an effective calcium-containing base for reaction with complexing acids21. The data in Table 6 is consistent with that finding. Thus, the third prior literature assertion (stating that only added calcium oxide or calcium hydroxide are appropriate for reaction with complexing acids) does not apply to this formulation under these conditions. Four-Ball EP weld loads were measured for Greases 15 and 16. As can be seen, Grease 16 had a value that was lower than Grease 15. This result implies that even though the thickener yield and dropping points were comparable, there is something different in the final reacted composition of these two greases resulting from the timing and temperature at which the calcium hydroxyapatite is added. Whatever the difference may be, it was not detected by FTIR, since the FTIR spectra of Greases 15 and 16 were identical. Greases 17 and 18 examined the effect of adding all the complexing acids before conversion but after the calcium hydroxyapatite had been added and allowed to thoroughly mix into the initial unconverted mixture. The acetic acid would have reacted almost immediately after its pre-conversion addition at ambient temperature23. As already explained regarding Greases 11A/B â€“ 14, the preconversion 12-hydroxystearic acid would not be expected to significantly react with basic components until it began to melt as the mixture was heated to the conversion temperature (88 C).
Comparing the results of Greases 15 and 16, there were no significant differences in thickener yield or dropping point regardless of whether the calcium hydroxyapatite was added before or after conversion. In this regard, calcium hydroxyapatite appears to be different from the added calcium carbonate used in Greases 1 and 2 where the first chemistry modification was used. Nonetheless, the first prior literature assertion (concerning the adverse effect of calcium-containing bases present during conversion) does not apply to this formulation under these conditions. Although not part of the work reported herein, previously reported work has shown that calcium hydroxyapatite can
Comparing Grease 17 (pre-conversion 12-HSA) with Greases 15 and 16 (postconversion 12-HSA), where the same overbased sulfonate A2 was used, the pre-conversion addition of the two complexing acids improved thickener yield, although the dropping point was reduced. Once again, this result demonstrates that such process changes do affect the chemical structure of the resulting grease. Looking at the results in Tables 6 â€“ 7, the fourth prior literature assertion (concerning thickener yield improvement when adding at least some of the complexing acids pre-conversion) once again appears to apply in varying degrees depending on the specific details of the formulations under these conditions.
- 23 NLGI SPOKESMAN, MARCH/APRIL 2018
The thickener yield was slightly better for Grease 17 (preconversion 12-HSA; sulfonate A2) compared to Grease 18 (pre-conversion 12-HSA; sulfonate B). This indicates that overbased calcium sulfonate A2 may provide slightly more thickening than overbased calcium sulfonate B when the calcium hydroxyapatite chemistry is used as in these greases. This is the opposite of what was observed when using the first chemistry modification as described earlier in this paper. Thus, the relative thickener effectiveness of different 400 TBN overbased calcium sulfonates can depend on various details of the grease chemistry approach used. The dropping point of Grease 18 was higher than Grease 17. A final set of four greases was prepared to evaluate the effect of the pre-conversion addition of both calcium carbonate and calcium hydroxyapatite. The amount of calcium hydroxyapatite was set at a level such that the total hydroxideequivalent basicity was insufficient to react with all added acids (DDBSA and complexing acids). The calcium carbonate was added to provide additional basicity for reaction with the acids. These four greases could be considered to be a combination of the two previously described chemistry modifications. All four greases used overbased calcium sulfonate A2. These four greases were made according to the general process profile provided in Figure 4.
All four of these greases used 12-HSA, acetic, and phosphoric acids as complexing acids. Greases 21 and 22 also used boric acid as a fourth complexing acid with Grease 22 having more than twice the amount of boric acid used in Grease 21. This was the only difference between Greases 21 and 22. For Grease 19, all complexing acids were added after conversion; for Greases 20 â€“ 22, 40% of the 12-HSA and acetic acids were added pre-conversion after addition of the calcium bases with the remainder added post-conversion. Phosphoric acid was always added after conversion and after any remainder of 12-HSA and acetic acid had been added and allowed to react. When boric acid was added, it was always added post-conversion after any remainder of 12-HSA and acetic acid, but before the phosphoric acid. Also, for Greases 21 and 22, only half the total amount of calcium carbonate was added before conversion. The remainder was added after the grease had converted, reached top processing temperature, and cooled down to 121 C (250 F). Final compositions and test data are provided in Table 7.
- 24 VOLUME 82, NUMBER 1
As can be seen, the effect of adding all or some of the 12-HSA and acetic acid before conversion did improve yield, as shown by the final concentration of the overbased sulfonate A2 in Greases 20 and 21 compared to Grease 19. Similarly, dropping point was improved. This improvement in thickener yield was observed regardless of whether boric acid was used (Grease 21) or not (Grease 20). Thus the combined pre-conversion addition of calcium hydroxyapatite and calcium carbonate appears to provide a combination of benefits previously observed when each of the two calcium-containing bases were separately added. By comparing Greases 21 and 22 and accounting for the difference in worked penetrations, it appears that increasing the level of boric acid provided little if any improvement in thickener yield. Dropping point may have actually decreased. Four-Ball EP weld loads were excellent for the three greases in Table 7 (620 kg to >800 kg), although boric acid may have contributed to the effect. Finally, the overall superior thickener yield data of Table 7 compared to the earlier greases continues to show that the first and third prior literature assertions are not valid for these formulations and processing conditions. However, the fourth prior literature assertion is valid for those formulations and processing conditions.
The next two sections provide information on how the two previously described calcium sulfonate-based grease chemistry modifications can be applied to lubrication in two specific commercial applications: open gears and braided wire ropes. Commerical Application: Open Gear Lubricant Performance requirements/guidelines for lubricants used in open gear applications are described in what is probably the most important industrial gear lubricant specification in North America: ANSI/AGMA 9005-E02. Additionally, various OEMâ€™s have established specifications reflecting their equipment needs. Viscosity is one of the most obvious features that becomes apparent when examining these specifications. The viscosity guidelines or requirements vary considerably. The primary reason is that there are different gear types, lubricant types, and lubricant application systems that make a single viscosity requirement impossible. This information as well as information on other performance requirements have been reviewed in several recent papers22,23, and will not be repeated here. Calcium sulfonate-based greases have been previously proposed as a good choice for open gear lubrication24. Their
- 25 NLGI SPOKESMAN, MARCH/APRIL 2018
intrinsically good load carrying, antiwear, and shear stability properties make them a reasonable choice in such applications. A formulation using chemistry modification No. 2 was developed for an open gear application where the lubricant was delivered to the gear teeth by high pressure nozzles. A first iteration product was formulated based on the composition of Grease 21. The only significant differences were as follows: 1. A 40/30 (wt/wt) blend of a 2000 SUS (382 cSt at 40 C) naphthenic base oil and a high molecular weight polybutene was used instead of a 600 SUS solvent neutral Group I base oil. The polybutene had a kinematic viscosity of 4400 cSt at 100 C. 2. The base oils were added in sufficient amount to provide an unworked penetration of about 380. 3. Pre-conversion calcium hydroxyapatite was supplemented by added calcium hydroxide such that the calcium hydroxyapatite provided 25% of total added hydroxide-equivalent basicity for reaction with complexing acids. 4. The final product was not milled. This was done intentionally so that the final product with or without diluent evaporative solvent would be easier to pump and inject onto the gear teeth. The high pressure injection followed by the high pressure shearing by the gear teeth would be expected to further thicken the product similar to what the lubricant would have experienced if milled. The resulting formulation was tested to determine various performance-related properties. Results along with performance target values are provided in Table 8.
As can be seen in Table 8, the product had good performance, especially considering that it had no performance enhancement beyond what was provided by its overall Grease 21 composition. However, the FZG scuffing load was below the targeted level. In order to improve the load carrying properties and introduce other important properties not yet present, this formulation was modified as follows:
1. Boost FZG load carrying properties by further inclusion of oil-soluble and oil-insoluble EP/AW additives. Some of these additives provided additional functionality.
2. Addition of antioxidants (which had thus far intentionally not been used).
3. Addition of passivating additives to counter the effect of active sulfur introduced in some of the oil soluble EP/AW additives.
4. Addition of dye (non-functional, cosmetic).
All additives were added after the grease had reached its top temperature and had cooled to below 121 C (250 F). The generalized composition of this modified formulation is provided in Table 9. Test results are provided in Table 10. - 26 VOLUME 82, NUMBER 1
With the targeted bench test properties achieved, the formulation was cut back with an 8% addition of an evaporative solvent blend. This was done for two reasons: 1. Improve the pumpability/sprayability of the gear lubricant onto the open gearing teeth, in accordance with the requirements of the lubricant delivery systems of two targeted potential trial locations. The use of such diluent solvents is a common practice when using grease-based open gear lubricants24. 2. Provide rapid evaporation to help further thicken the lubricant on the gear teeth.
Unfortunately, no field performance data are yet available. Resulting data, once available, may become the part of a future paper. Commercial Application: Braided Wire Rope Lubricant Braided wire ropes are commonly used in mining and marine applications. A braided wire rope consists of many individual steel wires that are helically coiled into a braided structure. Braided coils of these steel wires are then helically braided in multiple layers around a core. The core may be another helically braided grouping of steel wires, or it may be a non-metallic flexible material. When the conveyance or
- 27 NLGI SPOKESMAN, MARCH/APRIL 2018
payload being moved is sufficiently heavy, braided wire ropes can be several inches in diameter with several layers of braided bundles of the individual steel wires. Figure 5 provides an endon schematic and a picture of a braided wire rope. During the movement of the conveyance or payload, the braided wire rope is coiled and uncoiled from a large spool-like hoist. Similarly, the braided wire rope bends around a pulleylike sheave wheel, depending on the configuration of the actual application. Such movement of the braided wire rope will cause rubbing of the individual steel wires and the braided bundles of steel wires. In the absence of sufficient lubrication, progressive wear occurs that eventually compromises the strength of the wire rope and shortens its useful life. Figure 6 provides a picture of a typical wire rope hoist in operation. Wire ropes can also experience corrosive environments due to humidity and exposure to water (fresh and salt). In some mining applications, ground water can have a pH value of 3.0 or lower. This extremely acidic environment will further aggravate the potential for corrosion. Wire rope lubricants are applied to protect wire ropes and extend their useful life. Some of the performance requirements of a wire rope lubricant include the following: 1. Protect wire strands from wear and corrosion. 2. Be pumpable from the original container to lubricant applicators without the use of external heating devices. 3. Provide a barrier against intrusion of water and other contaminants.
4. Neutralize acidic contaminants. 5. Remain on the wire rope without sling-off during use. 6. Remain flexible and pliable during cold weather instead of becoming hard and brittle. Although the above list is not a complete one, it does suggest that a properly formulated calcium sulfonate-based grease might provide the basis for excellent performance as a wire rope lubricant. Although either of the two chemistry modifications previously discussed might provide a good choice, the calcium carbonate-based chemistry modification No. 1 was chosen. Furthermore, a simple calcium sulfonate grease approach was chosen. This choice was made for three reasons: first, such an approach would have a higher TBN value since none of the calcium carbonate would have been neutralized by complexing acids; second, the higher overbased calcium sulfonate concentration would enhance prtoection against ferrous corrosion; and third, the simple calcium sulfonate grease structure would be intrinsically more tacky and adherent than otherwise similar calcium sulfonate complex formulations as described in this study. A simple calcium sulfonate grease formulation was developed with the generalized composition as provided in Table 11. This formulation was made according to the process profile of Figure 1 with all the calcium carbonate added before conversion. The naphthenic and polybutene base oils were the same as used in the previously described open gear lubricant formulation. All additives were added after the grease had reached its top temperature and had cooled below 121 C (250 F).
- 28 VOLUME 82, NUMBER 1
The formulation was augmented with an 8% addition of a blend of two evaporative solvents, one of which had a significantly higher evaporation rate than the other. This was done for similar reasons as explained in the previous section on open gear lubricants. Additionally, the two solvent blend was used so that one solvent would evaporate quickly while the other would evaporate more slowly, allowing it more time to carry the lubricant to the interior of the wire rope. The solvents were also chosen so as to be acceptable with regard to Canadian regulatory requirements. Test data are provided in Table 12, wherein all data is for the solvent-free formulation unless otherwise specified.
- 29 NLGI SPOKESMAN, MARCH/APRIL 2018
The bottom two tests in Table 12 need explanation. First, the brush and impact test is a procedure whereby a 0.5 inch diameter braided wire rope segment is cleaned and then painted with a thin coat of the solvent cut wire rope lubricant. The wire rope segment is clamped on one end and vertically suspended for 30 minutes to allow the solvent to evaporate. Then it is removed and both ends are cleaned so that it can be handled. The wire rope segment is then repeatedly brought down as hard as possible against a square wooden frame that sits on white paper. The complete lack of flinging of any lubricant from the wire rope onto the white paper below is considered a pass. This test is commonly used in the mining industry as a method to determine if a wire rope lubricant will remain on the wire rope during use. While this test is crude, it has proven to be a good screening tool. Second, the freezer flex test similarly involves painting and suspending a wire rope segment. Then it is stored in a cold chamber at -22 C for three days. After that duration, it is removed and repeatedly flexed by hand into a horseshoe configuration. A passing result requires that the lubricant film remains pliable and shows no signs of hardening or cracking. The wire rope lubricant formulation in Tables 11 and 12 was tested in more than ten Canadian mines. Results have been good. In one specific location, the mine operated a 10-foot double drum hoist capable of operating to a 4,200 foot depth. The wire ropes were inspected by the Canadian Ministry of Mines every six months as required in all Canadian mines The previous wire rope lubricant used in that mine had been a viscous asphaltic product. The mine had been experiencing what they considered to be shorter than desired rope life. Each time a wire rope needed to be replaced, the hoist had to be shut down for two days, effectively stopping all mining activity. The new wire rope lubricant extended the life of the in-service wire ropes by an estimated one year, primarily due to slowing of corrosion (that had already been occurring on the in-service ropes) due to acidic water. No sling-off was observed once the correct application rate had been established. When the new product was first applied to freshly cleaned ropes and began to penetrate therein, actual displacement and explosion of water (that had been entrained previously in the in-service wire rope when the other lubricant was in use) was visually observed. Figure 7 shows two pictures of the old asphaltic product being removed from
the wire rope by the equipment that is designed for that express purpose. In another mine, the previous wire rope lubricant was a synthetic oil fortified with oil-soluble sulfurized additives. The 400 lb. drums of this product had to be heated to 93 C (200 F) using band heaters so as to be able to pump the product to the applicator equipment. This was due to the extremely high viscosity of that product at ambient temperatures in the hoist room. The new wire rope lubricant did not require any such heating. No sling-off was observed once the correct application rate had been established. Problems experienced during use of this new wire rope lubricant formulation have primarily been due to misapplication. As already mentioned, specialized equipment must be used to clean the old lubricant off the ropes before applying the new lubricant. Special equipment is needed to apply a thin, contour-fitting film of the new lubricant. When improper application equipment was used, over-lubrication nearly always resulted. Even when the correct application equipment was employed, users often had to significantly reduce the application rate from the previous setting to avoid applying an excessive amount of the new lubricant. When this was necessary, it was usually due to the previous lubricant having a much higher viscosity. The thin contour-fitting coating of the new wire rope lubricant was difficult to see in some mines where they had previously used an opaque black asphaltic product. Typical application of black asphaltic wire rope lubricants results in a black pipe-like, semi-solid coating where the outer strand and groove structure of the wire rope is no longer visible. In order to determine that the new lubricant was adequately applied, the outer surface of the wire rope was touched with a white cloth. Clear blue residue on the cloth that matched the pattern of the outer groove design showed that the new lubricant was present. Another problem that was encountered involved the use of new wire ropes. New wire ropes come with a wax-like coating to protect it from corrosion until the time of installation by the user. If that initial coating is not correctly removed (or not removed at all), no wire rope lubricant will properly adhere. Initial on-site guidance was usually required in order to insure that instructions on proper wire rope preparation and lubricant application were followed.
- 30 VOLUME 82, NUMBER 1
The following conclusions are supported by the results discussed in this paper. 1. When making a calcium sulfonate-based grease, adding either calcium carbonate, calcium hydroxyapatite, or both calcium carbonate and calcium hydroxyapatite before conversion does not impair the conversion process, and does not have an adverse effect on the measured test properties of the resulting grease. 2. The deleterious effect of too much pre-conversion water or prolonged presence of that water after conversion on thickener yield and dropping point can still occur when using the new chemistry modifications described in this paper. For best results, pre-conversion water should be removed from the grease by evaporation as soon as practically possible. 3. Calcium carbonate, when added before or after conversion, is an effective base for reaction with complexing acids when making calcium sulfonate-based greases. Pre-conversion addition is preferred for optimum thickener yield and dropping point. 4. When properly selected and formulated, the two new chemistry modifications described in this paper (adding calcium carbonate and/or calcium hydroxyapatite before conversion) can be used to formulate effective wire rope lubricants. 5. When properly selected and formulated, the two new chemistry modifications described in this paper can be used to provide lubricants that show excellent potential for use in open gear lubrication based on laboratory test data. Verification of this potential open gear lubricant performance will require documented field testing. 6. When introducing significantly new and different lubricants into existing field applications, initial on-site guidance and monitoring are necessary to ensure proper performance evaluation. 7. The two new chemistry modifications described in this paper continue the growing trend of increased usefulness of calcium sulfonate-based greases in an ever-expanding scope of applications.
The author gratefully acknowledges Joe Garza for his work in preparing and testing the greases discussed in this paper. 1 Waynick, J. A. “Days of Future Passed: A Critical Review of the Development of Highly Overbased Calcium Alkylbenzene Sulfonates”; NLGI 83rd Annual Meeting, Hot Springs, VA, June 2016.
2 McMillen, Richard L. “Basic Metal-Containing Thickened Oil Compositions”; U.S. Patent No. 3,242,079, 1966. 3 Muir, Ron; Blokhuis, William “High Performance Calcium Borate Modified Overbased Calcium Sulfonate Complex Greases”; U.S. Patent No. 4,560,489, 1985. 4 Barnes, John F. “Calcium Sulfonate Grease And Method Of Manufacture”; U.S. Patent No. 5,126,062, 1992. 5 Olson, William D.; Muir, Ronald J.; Eliades, Theo I.; Steib, Thomas “Sulfonate Greases”; U.S. Patent No. 5,308,514, 1994. 6 Olson, William D.; Muir, Ronald J.; Eliades, Theo I. “Sulfonate Grease Improvement”; U.S. Patent No. 5,338,467, 1994. 7 Mackwood, W.; Muir, R. “Calcium Sulfonate Grease - One Decade Later”; NLGI Annual Meeting, 1998. 8 Fish, Gareth; Ward Jr., William C “Calcium Sulfonate Greases Revisited”; NLGI 78th Annual Meeting, Palm Desert, CA, June, 2011. 9 McMillen, Richard L. “Basic Metal-Containing Thickened Oil Compositions”; U.S. Patent No. 3,372,115, 1968. 10 McMillen, Richard L. “Process For Preparing Lubricating Grease”; U.S. Patent No. 3,376,222, 1968. 11 McMillen, Richard L. “Process For Preparing Thickened Compositions”; U.S. Patent No. 3,377,283, 1968. 12 McMillen, Richard L. “Non-Newtonian Colloidal Disperse System”; U.S. Patent No. 3,492,231, 1970. 13 Asseff, Peter A., et. al. “Organic Alkaline Earth Metal Complexes and Method of Making Same”; U.S. Patent No. 2,616,905, 1952. 14 Asseff, Peter A., et. al. “Organic Alkaline Earth Metal Complexes and Method of Making Same”; U.S. Patent No. 2,616,924, 1952. 15 Asseff, Peter A., et. al. “Methods of Preparation of Superbased Salts”; U.S. Patent No. 2,695,910, 1954. 16 Mastin, Thomas W. “Oil Soluble Metal Containing Compositions and Process For Making Same”; U.S. Patent No. 2,971,014, 1961. 17 Waynick, J. A. “Calcium Hydroxyapatite Based Calcium Sulfonate Grease Composition and Method of Manufacture”; U.S. Patent No. 9,458,406, 2016. 18 wartz, Charles J.; Hardy, Bryant J. “Process for the Preparation of Over-Based Group 2A Metal Sulfonate Greases and Thickened Compositions”; U.S. Patent No. 5,190,678, 1993. 19 Hunt, Mack W. “Method for Preparing Highly Basic Grease and Rust Inhibiting Compositions”; U.S. Patent No. 3,816,310, 1974. 20 Budavari, Susan (Ed.) The Merck Index, 11th Edition; Merck & Co., Inc.; p. 1676, 1989. 21 Waynick, J. A. “Calcium Sulfonate Complex Greases Using Calcium Hydroxyapatite as a Hydroxide-Containing Basic Reactant”; NLGI 82nd Annual Meeting, Coeur d’Alene, ID, June, 2015. 22 Ludwig, Lawrence G. “Methods of Application for Open Gear Lubricants and Their Selection”; NLGI 78th Annual Meeting, Palm Desert, CA, June 2011. 23 Lorimor, John J. “Understanding Open Gear Lubricants: Product Design Considerations”; NLGI 79th Annual Meeting, Palm Beach, FL, June 2012.
The Typical Application of Calcium Sulfonate Complex Greases in Steel Mills By: Li Jiwei, Cheng Shutian, Zhao Wei, Wu Baojie Tianjin Branch, SINOPEC Lubricant CO., LTD.
Abstract The production process in steel mills is pretty long with numerous equipment exposed to a variety of working conditions that require different greases. For example, some equipment exposed to large amounts of water for extended periods of time require grease with excellent water resistance properties. In the areas of high ambient temperature and long re-lubricating intervals, the grease requires thermal and oxidative stability. In alkaline environments, the grease needs excellent protective properties. Calcium sulfonate complex grease (CSCG), with its comprehensive and excellent properties, is increasingly popular in the steel mill industry. Certain properties of CSCG can be further improved by formulation and process design to meet requirements of grease on different equipment in steel industries. Typical data for several CSCGs will be presented in this paper. In addition, their application performance in the equipment in wet, rusty, high temperature, alkaline environments and open gears will also be discussed. Introduction Machines and equipment in the steel industry are generally operated in the conditions of high temperature, high load, vast water spraying and continuous working. The typical working conditions are • High temperature - The temperature at the of bottom of an iron-making blast furnace is 1300-1500 °C, and at its top the temperature is 400-600 °C. The temperature of a secondary cooling area of continuous casting is 800-900 °C, and the billet temperature during hot rolling is 850-1000 °C. The high temperature radiates and conducts heat to lubricated parts. • Water spraying - A large amount of water spray occurs on billet steel on roller bearings, rollers and bearings of hot rolling, on pinch rolls and guided rolls in secondary cooling areas of continuous casting. High pressure water is used to remove phosphorus from other equipment. • Dust – There are great amounts of dust, mainly the smoke,
iron slag, steel slag and iron scale generated due to fuel burning. • Loads - Heavy loading and impact loads are applied during the working process to working roll bearings of rolling mills, shearing machines, rocking shear of continuous casting equipment, bearings of coiling machines, exposed gears and other equipment. • Operations - Continuous operations at steel enterprises are common. Production equipment can be operated stably for long periods of time. In order to meet the requirement for high reliability of metallurgical equipment, grease must withstand the test of these working conditions. In recent years, CSCG started to attract the attention of the grease industry by its comprehensive, excellent performance such as excellent high temperature performance, mechanical stability, colloidal stability, extreme pressure and anti-wear performance, water resistance and excellent corrosion resistance. There are a number of reports showing applications in industrial facilities under severe lubricating conditions at steel mills1-3. Certain properties of CSCG can be further improved by formulation and process design to meet requirements for grease on different equipment in the steel industry. Typical data of several CSCGs will be presented in this paper. Application of CSCG in the Presence of Water Rolling mills and continuous casters equipment consume large amounts of grease in the steel industry, under wet working conditions. Refer to Table 1 for typical data for CSCG for wet applications. A hot rolling mill is the key equipment in a hot rolling plant, and bearings in rolling mills are just like joints in humans. Today, the steel industry is committed to continuous production. If the rolling mill bearings burn, it will cause a huge economic loss or downtime. Therefore, it is very important to monitor the performance of grease used in a rolling mill’s bearings. Performance and trends of grease can be learned through the analysis and tests of samples.
- 32 VOLUME 82, NUMBER 1
The authors carried out a lengthy field application test in some 2250 hot rolling mill plants. CSCG application performance in rolling bearings, included the effect of water on properties of CSCG, was studied. Working conditions of rolling mill bearings are pretty harsh. Equipment has to operate under continuous shock, vibration, and exposure to significant amounts of water, as well as the impact of impurity invasion. Figure 1 shows the typical seven-rack fine rolling set in a hot continuous rolling mill. It can be seen that the bearing box is exposed in the environment with large amounts of water and moisture, and water and moisture may unavoidably penetrate into the internal part of bearings by permeating the seal, which causes negative effects on lubrication.
Considering the characteristics of rolling mill bearingâ€™s working conditions, the authors will focus on comparing the changes of consistency, wear resistance, and extreme pressure performances of used greases, as well as their consumption and bearing temperature changes. Bearing is the open type, and sampling point is shown in Fig 2. The sampling point is inside the seal and close to the rolling elements. Eleven samples of CSCG with different water content were collected randomly from different bearings. Due to the limited sample amount, the grease consistency was measured with the 1/4 scale worked penetration test device.
- 33 NLGI SPOKESMAN, MARCH/APRIL 2018
Figure 3 shows the trend of penetration of used CSCG against water content. As the figure shows, the higher the water content of samples, the smaller the cone penetration value, which means the grease consistency was harder. If grease is too hard, then grease will cause high torque resistance. The poor fluidity will easily lead to uneven distribution of grease in the bearing, and grease will have difficulty reaching the roll neck and bearing inner circle. When the water content of this CSCG reaches to 40% and its consistency is 66 (0.1 mm), this grease slightly thick, but still has the good mobility. Figure 4 shows the variation trend of used CSCGâ€™s extreme pressure performance against water content. With the increase of water content, the four-ball weld load (PD) value is gradually reduced, which may result from concentration
decrease of component with the role of extreme pressure additive, such as calcite calcium carbonate. After heating to remove moisture from a sample, the PD value recovered to the original value of 400 kg. When the water content in CSCG increases, the PD value decreases and the lowest value is 160 kg. Even when the grease is saturated with water, the PD value is not less than 160 kg. This feature of CSCG effectively protects the operation of bearings and improves the reliability of bearing, so that the bearing can maintain good lubrication performance under the condition of high impact loads. Figure 5 shows the variation trend of four-ball wear scar diameter against water content of CSCG. From the Figure 5, we can see that when the water content is 7, 13, 14, and 16%, four-ball wear scar was between 0.38 and 0.42 mm. The wear
- 34 VOLUME 82, NUMBER 1
scar increased to 0.46 mm at 38 and 40% water content. Water had a relatively small effect on the wear resistance of this CSCG. The consistency change is small and the stickiness is kept well when CSCG is exposed to water, and it wonâ€™t be easily thrown out when bearings operate at high speed. Due to prominent water-resistance and comprehensive properties of CSCG, the re-greasing period of bearings of rolling mills is greatly prolonged, which reduces the manual grease adding frequency and charge of water treatment at the same time. The comparison of data before and after using CSCG in steel mills is shown in the following Table 2. Based on the statistics of many steel mills in China by the authors, the consumption amount of CSCG in bearings of rolling mills is only 30% of the amount of extreme pressure lithium, or 60% of complex lithium grease. Continuous casting is a process of steel production, and it directly influences the quality of steel rolling in the next procedure and finished steel materials. Therefore, it is especially important to guarantee normal and highly effective operation of continuous casters. A continuous caster uses a lot of grease, and equipment grease is crucial. There are many grease types for continuous casters in the steel industry in China, including extreme pressure lithium, complex lithium, and polyurea grease.
The consumption of grease is huge, and it is easily hardened or softened (it runs off at high temperatures, resulting in short time between maintenance). Through on-site application for many years, CSCGs show excellent performance that can reduce comprehensive usage cost and reduce equipment maintenance time. Figure 6 shows a typical continuous caster, and Fig 7 shows the roller bearings inside a continuous slab caster. It can be seen that grease inside bearing is full; in addition, color and consistency are kept well.
- 35 NLGI SPOKESMAN, MARCH/APRIL 2018
The pumping performance of CSCG is excellent without pipeline blocking. With CSCG, the grease usage amount may be reduced for continuous casters. And there is less blocking of roller bearings and spray nozzles for cooling water. The operation rate of continuous casting equipment is improved, too. CSCG will gradually become the mainstream grease used for continuous casters. Due to excellent water resistance properties, CSCG is not only applied to continuous casters and bearings of roller mills, but also to other equipment that are washed with water or stand in water. Application of CSCG in Alkaline Environment The CSCG in Table 3 has excellent alkaline resistance properties. In the alkaline washing environment in a cold rolling plant, the bearings of drying rolls are surrounded by alkaline smog, from a mixed solution of 3-5% KOH and NaOH. The previously adopted extreme pressure lithium grease may soften and run off rapidly, resulting in bearing block. A 5% KOH strong alkaline solution was prepared, and added (20 and 40%) to grease; then, the roller test was conducted by ASTM D1831 for 16 h. Grease consistency was measured before and after the test. The consistency of the grease with 20 and 40% solution changed by -4 and -15 (0.1 mm), respectively. Using CSCG on site solved the problem of grease thinning inside bearings after being exposed to alkaline solution. Application of CSCG to Protect Parts Excellent rust-resistance property of CSCG should be attributed to the strong polarity property of SO32- in the special structure of raw material so that it can be easily attached on metal surface. Also, the high alkaline value can neutralize acid materials generated due to oil oxidation and resist contact of
oxygen and moisture with metal surface, so that it has excellent rust resistance properties. Due to the excellent rust resistance properties, CSCG is widely applied in steel pipe production plants. The storage and transport of petroleum casing pipe are mainly in exposed environments, just as Fig 8 shows. Protective grease is coated on the joints of petroleum steel pipes and external screw threads. The grease shall have excellent high and low temperature properties and rust resistance properties to meet requirements for protection and lubrication during the storage and transport processes in cold winters, hot summers, rain, salt mist and other environmental conditions. Steel pipe manufacturers require protection of petroleum casing pipe screw threads. It is required that screw thread grease should have excellent brush coating and overlay properties; therefore, consistency is generally NLGI grade 0 or 00. Traditional greases may thin after being exposed to water, and their rust resistance properties will be worsened. In addition, casing pipe screw thread rusts easily in high and humid weather. The CSCG provides an excellent solution for steel pipe production enterprises. The salt mist test time can be 4000 h through special formulation design and adding rust-resistance additives. Refer to Table 3 for rust-resistance properties. Figure 9 shows the effect of using CSCG to protect petroleum casing pipe screw threads for 1 year. Application of CSCG to High Temperature Parts The compatibility of CSCG and specific synthetic oils is excellent, and Y. Kimura selects PAO to prepare CSCG with excellent low temperature and comprehensive properties4. In order to improve the usage effect of grease at high and low temperatures, the author uses alkyl naphthalene as base oil to prepare CSCG with excellent low temperature and comprehensive properties. Refer to Table 4 for typical data
- 36 VOLUME 82, NUMBER 1
for CSCG made from alkyl naphthalene as base oil. Such kind of grease has comprehensive and excellent high temperature consistency maintenance capacity and oxidation resistance lifespan, extreme pressure wear resistance property, high temperature bearing lifespan and low temperature property. The roll table in front of the heating furnace is the typical environment with high temperature about 200 Â°C for a long time, and the temperature is higher when the furnace door is open. At high temperature, traditional grease is easily lost or coked, while the CSCG made from alkyl naphthalene as base oil has excellent application effects; in addition, the regreasing period of equipment is improved two-fold, and there is no obvious hardening or loss of grease at high temperatures. CSCG has broad application prospects for some parts at high temperature, such as: roll tables in front of and behind heating furnaces, roller bearings at the bottoms of annealing furnaces, and other parts.
- 37 NLGI SPOKESMAN, MARCH/APRIL 2018
Application of CSCG in Heavy Load Equipment Steel plants have various heavy load equipment such as support bearings of ladle turrets, clutches, exposed gears and other machines. CSCG has excellent extreme pressure and wear resistance properties, and it is extremely capable of being used in low speed and heavy load equipment. Open gears operate under severe conditions, often at their design limits. Severe conditions include extreme pressures, varying speed and contamination. Grease made with complex calcium sulfonate thickener, high viscosity base oil, and additives such as MoS2 can meet the requirements above. The product has excellent extreme pressure and wear resistance properties, which can form a thick oil film on the gear surface. The majority of exposed gear greases are applied by spray, and the minority are applied using an oil basin, requiring grease with excellent pumpability. It is shown in some studies that CSCG has excellent low temperature pumpability for exposed gears5. The author uses high viscosity base oil and adds solid additives to prepare CSCG, which has been used in many steel plants, and the usage effect in exposed gears of blenders and rotary kilns is good. Refer to Table 5 for typical data of CSCG used in open gears. Conclusions There are many types of equipment in steel mills, the working conditions are complicated and abominable, and there are a great many lubrication points. Calcium sulfonate complex grease, with its comprehensive and excellent properties, is being used more and more in steel mills. Certain properties of CSCG can be improved further by formulation and process design to meet requirements for greases on different equipment in the steel industry. The large amount of applications in steel mills shows that after CSCG is exposed to water, slight changes occur in consistency and properties. In addition, CSCG can reduce grease consumption and provide an excellent solution for equipment lubrication in steel plants.
References 1) Mackwood, W., et al, NLGI Spokesman, Vol.63, No.5, August 1999, 24-37.2. 2) M. Iwasaki, Y. Kimura, H. Youda and K. Takemura, The Case Studies of Industrial Applications of Calcium Sulfonate Complex Grease in Japan, presented at the NLGI 75th Annual Meeting Colonial Williamsburg, Virginia, USA, June 7 - 10, 2008. 3) Hocine Faci, Philip Booker, Martin Maass, Marcus Totten, Steel Mill Lubrication: Boosting the Grease Performance for Longer Bearing Service Life, presented at the NLGI 81st Annual Meeting Palm Beach Gardens, Florida, USA, June 14 -17, 2014. 4) Y. Kimura, K. Takemura, J. Araki, H. Kojima, Study of Synthetic Oil based Calcium Sulfonate Complex Greases, Presented at the NLGI 72nd Annual Meeting, San Antonio, Texas, October 30 – November 1, 2005. 5) Raymond Drost, Donald Howard, Huafeng (Bill) Shen, PhD, The Effects of Thickeners on the Low Temperature Properties of Open Gear Greases, presented at the NLGI 82nd Annual Meeting Coeur d’Alene, ID, June 6-9, 2015.
- 38 VOLUME 82, NUMBER 1
Join Us this year as we return to the stunning Coeur dâ€™Alene Resort June 9-12, 2018
Registration NOW OPEN Click here to register online
Novel Polymer Grease Microstructure and its Proposed Lubrication Mechanism By: S. Chatra, D. Muller, C. Matta, R. Thijssen, M. N. bin Yusof and M. C. P. van Eijk SKF Engineering & Research Centre Abstract
A novel polymer grease microstructure is revealed consisting of amorphous polypropylene nano-particles uniformly distributed in the base oil. The corresponding grease shows excellent mechanical stability and is not subject to irreversible shear thinning. It has a potential for use at extremely low start-up temperatures. Rolling bearing tests show excellent lubricating performance and the ability for enhanced lubricant film formation. It is proposed that base oil released from the grease carries nanoparticles into the rolling contact. Keywords: grease, polypropylene, TEM, cryo-SEM, microstructure, rolling bearings, lubrication mechanism, nanoparticles.
The microstructure formed by the thickener of lubricating greases plays an important role in the lubricating performance in rolling bearings. It typically correlates with the type and concentration of the thickener agent, as well as base oil type and viscosity. In turn, the thickener determines important grease properties, e.g., mechanical stability and rheological behavior -. Typically, metallic soaps form a coherent network of semi-crystalline microfibres , while other thickener types may crystallize in spherical, plate-like or rod-like configurations . An alternative technology using a polypropylene thickener was presented previously by SKF , showing enhanced lubricant film formation and friction reduction . Due to the risk of mechanical degradation of the polypropylene thickener , improvement is desirable to prevent grease softening. This investigation focuses on a new polymer grease insensitive to mechanical degradation owing to an alternative synthesis process . The thickener structure of the new polymer grease is characterized, and its lubrication performance is investigated in Spherical Roller Bearing (SRB) testing.
2. Material and Methods
2.1. Greases for thickener structure analysis Polypropylene (PP) polymer grease is synthesised in a twostep process. First, polypropylene dissolved in base oil at 180 – 200 °C is rapidly cooled to 80 °C or below in less than 30 s. Second, the material obtained is processed at 80 ºC by prolonged shearing at low intensity using, e.g., a planetary mixer. During processing, the initial material, which is relatively stiff (NLGI>4) is softened gradually over 2 – 8 hours until an NLGI 2 – 3 grade grease is obtained having an oil separation typically in the range of 3-6% (as per IP 121). The grease composition in this study consists of 13 wt% polymer in polyalphaolefin (PAO) (viscosity 68 cSt at 40 ºC). The polymer consists of 95 wt% polypropylene (homopolymer, 50,000 <100,000) and 5 wt% copolymer (polyethylene-polypropylene block copolymer, >200,000). The grease reaches a stable NLGI 2 consistency during processing, with a worked penetration of approximately 265 (0.1 mm). Grease structure analysis was performed on the polypropylene (PP) polymer grease and compared with a reference NLGI 2 lithium 12-hydroxystearic acid (12-HSA) grease (Li - R). The latter was prepared in the laboratory, consisting of 9.6 wt% thickener in the same PAO base oil. Scanning Electron Microscopy (SEM) was used to investigate the residual thickener structure following base oil extraction from grease samples by rinsing with a volatile hydrocarbon solvent. Cryogenic Scanning Electron Microscopy (cryoSEM) was used to visualize the in-situ thickener structure, i.e., the thickener distribution in the base oil environment  . Transmission Electron Microscopy (TEM) was used to characterise the atomic structure, notably crystallinity, of the PP grease thickener. For rheological analysis, two commercial lithium complexPAO greases (Li - I and Li - II) possessing good mechanical stability were used for reference. For Spherical Roller Bearing
- 40 VOLUME 82, NUMBER 1
(SRB) testing, the PP grease was additized to accommodate wear protection. Bearing testing was performed comparing the additized PP grease and the base PP grease. In addition, a commercial high-speed grease (Li - III) and an extreme pressure grease (Li - IV) were tested for reference. The main characteristics of the investigated greases are summarized in Table 1. The relative film thickness of the PP grease was investigated through the use of capacity measurements. Grease rheology was investigated on a DHR-2 rheometer from TA Instruments, characterising shear viscosity according to DIN 51810-1, and shear stability according to DIN 51810-2. The yield stress of the greases was determined on an MCR 302 rheometer from Anton Paar. Measurements were carried out using a 25 mm diameter parallel-plate fixture with a smooth stainless steel surface. 2.2. Bearing testing Full bearing tests were performed using a modified SKF R2F test method (obsolete DIN 51806). The test rig consist of a radially loaded shaft mounted with two test bearings (SRB 22312 E C3) in housings without seals, and two support bearings (ACBB 2310 E-2RS1TN9), see Figure 1. The bearing load, 8.3 kN, corresponds to a maximum inner ring contact pressure of 1.1 GPa. Bearings are pre-greased (50 g) and housings partially filled with grease (150 g) corresponding to a filling degree of 30%. Overall grease performance was evaluated by measuring the self-induced temperature (outer ring) at 1000-4000 rpm over 240 h (10 days), see Table 2. After 24 h at 3,000 rpm, a fan was used to suppress overheating of the support bearings, thereby lowering the self-induced temperature of the test bearings.
Grease performance was benchmarked using the high-speed reference grease Li-III. Film thickness was evaluated at low speed and at a constant temperature of 80 °C. The procedure comprised a running-in phase of 100 h at 250 rpm, followed by 82 speed cycles at 0 – 250 rpm with a duration of 176 h, as detailed in Table 3. Lubricant film formation was evaluated individually for both test bearings using a LubCheck system. LubCheck measures the electrical capacitance in the rolling contact originating in the presence of an electrically insulating lubricant film. LubCheck provides, after filtering the raw signal, an averaged electrical potential (V) representative of the electrical conductivity of the rolling contact. The value varies from 0 V, representing metallic contact, to a maximum (preset) value representing an infinite lubricant film. Speed was changed at 1 rpm/s during cycles, i.e., requiring a speed ramp of 4 min, 9 s to complete a maximum increase/decrease of the rotation speed. As a result, the variation in film thickness could be monitored accurately. The LubCheck signal is converted to a mean lubricant film thickness through a calibration step by repeating the test procedure using PAO base oil (viscosity 400 cSt at 40 °C). The empirically obtained curve is fitted to the theoretical mean film thickness of the PAO oil as a function of speed, using the bearing geometry and base oil viscosity as input parameters. Using the calibration step, differences in permittivity between reference oil and greases are not considered. The calibration represents simplified assumptions regarding film thickness, however provides a direct comparison of film building behavior of the experimentally tested greases and the reference PAO base oil.
- 41 NLGI SPOKESMAN, MARCH/APRIL 2018
- 42 VOLUME 82, NUMBER 1
3. Results and discussion
3.1. Grease structure characterisation Figure 2 shows SEM micrographs comparing the thickener structure of the PP grease before and after the processing step during synthesis. The structure before processing is highly condensed, whereas the processed structure is more porous. On a smaller length scale, a nodular morphology is visible in both cases. Identical nano-scale particles of 10-15 nm diameter are present in the initial and in the processed materials; these must, therefore, form during phase separation of polypropylene in base oil and remain after processing.
The particles appear spherical and homogeneous in size and distribution. SEM micrographs of the lithium grease Li-R, in Figure 3, show a thickener consisting of thin elongated fibres with a substructure of coiled helices. In turn, these consist of semi-crystalline material, as has been reported previously . Clearly, the polymer thickener has structural elements on a nanoscale, much smaller compared to the lithium soap thickener. It should be noted that after removal of the base oil from the sample material for SEM analysis, the thickener fibres are no longer dispersed in a reticular form and appear highly concentrated.
- 43 NLGI SPOKESMAN, MARCH/APRIL 2018
Figure 4 shows TEM images of the PP grease after processing, deposited on a copper grid. The TEM image of the thickener associated with the electron diffraction pattern clearly reveals that the polymer thickener has an amorphous structure. An Energy Dispersive X-Ray (XRD) analysis of the structure reveals that it is composed completely of carbon (not shown in this article). The in-situ microstructure of the above greases is shown in Figure 5, using cryo-SEM analysis of freeze-fractured samples . The fracture surface of Li-R shows isolated, coiled fibre helices. Observation of complete fibres is limited by the necessity to align the fracture angle with the fibre direction. The processed PP grease shows a very distinct microstructure, consisting of a homogeneous distribution of particles in PAO base oil. The particles are spherical, with a diameter of 10-15 nm, corresponding well with the SEM analysis. No visible connection is identified between the particles. It may be inferred that due to their small size, the particles remain intact, or at least visible, following the freeze-fracture process. Overall, electron microscopy reveals a PP grease microstructure composed of homogeneously dispersed, amorphous, solid polypropylene particles of 10-15 nm diameter. Rheological investigation (discussed below) offers clues, not regarding the nature of the interaction, but regarding the extent of the interaction inside the PP grease. It is clear that in comparison with the lithium grease (fibre network) and also other polymer greases previously reported, the microstructure of the PP grease presented here is radically different.
the grease before and after processing. Before processing, fibre-like connections can be seen in the fracture zone. This is an indication of strong internal cohesion in the thickener structure before processing. The enlarged image clearly shows that this is the result of cohesion between particles. After processing, the cohesion has largely disappeared. This supports the cryo-SEM observation that particles are no longer physically connected after processing. The in-situ structure of the PP grease before processing could not be investigated due to difficulties freeze-fracturing this material.
Figure 6 shows SEM micrographs of fractures in the PP thickener (after removal of the base oil), comparing - 44 VOLUME 82, NUMBER 1
3.2. Grease properties The roll stability test (ASTM D1831) resembles the processing step at low shearing intensity during polymer grease synthesis, notably over an extended duration. The polypropylene grease investigated was processed to a worked penetration of 269 (0.1 mm, NLGI grade 2 consistency). Additional processing will result in limited, further softening. The current composition was targeted at an NLGI 2 grease, while balancing moderate processing time and good mechanical stability. After roll stability testing for 50 h at 80 °C, the worked penetration increased by 42 from 269 to 311 0.1 mm, and additized grease work penetration was increased by 35 from 269 to 304 0.1 mm, see Table 1. At this point, it can be expected that nanoparticles in the thickener structure are fully separated. It is likely that interparticle interactions providing grease stability are related to steric interactions between polymer chains protruding from the nanoparticles. This could be further promoted by the high molecular weight copolymer fraction in the polymer grease. The “stabilized” consistency, obtained by extended low intensity shearing, depends on the concentration of particles. By increasing thickener content, the stabilized consistency will shift upwards. Drastically increasing the shearing intensity during processing, e.g., by homogenisation, may degrade interparticle interactions, or possibly, the nanoparticles themselves. In bearing lubrication, there is high shear stress only close to or inside the rolling contacts. The lubrication mechanism should, therefore, not depend on mechanical thickener degradation to replenish the rolling contact. The flow properties of the polymer grease and lithium complex greases were investigated as a function of shear rate at 25 °C using DIN 51810-1. The transition from elastic solid to a viscoelastic liquid occurs when exceeding the yield stress, τγ. In Table 4, the yield stress is shown as obtained from the shear stress at the maximum viscosity. Beyond this point, the viscosity decreases due to breakdown of internal cohesion with increasing stress. As can be seen, Li-I shows the lowest yield stress (134 Pa), followed by polytetrafluroethylene (PTFE) grease (143 Pa) and Li-II (219 Pa). This follows the trend in cone penetration data. Surprisingly, the PP grease has a much higher yield stress (453 Pa) but a cone penetration value similar to the other greases. This may be beneficial to retain a grease reservoir in bearings close to the rolling contact, or to prevent grease leakage.
Oscillatory shear was applied to characterise the Linear Viscoelastic (LVE)behavior of the PP grease at low shear rates, in the region before the grease yields. The measurements are performed by applying an oscillatory amplitude shear sweep, τosc, ranging from 1 to 10,000 Pa and keeping the angular frequency constant, ϖ= 10 s-1 as defined in DIN 51810-2. Characterized by the storage G’ and loss G” moduli, the LVE represents the elastic and viscous parts of the grease, respectively. In Figure 7, the stability of the PTFE greases is compared in the LVE domain at 40 and 80 °C. The PTFE grease is composed of PTFE thickener and synthetic fluorinated polyether base oil and is NLGI grade 2. Good bearing performance requires G’ >> G” in the LVE region, essentially giving the grease’s inherent stiffness. At the cross-over stress, τco, the material is already in a state of flow. Clearly, the PP grease shows good stability in the LVE region and very similar behavior at 40 and 80 °C. Low-temperature properties of the PP grease were investigated using the low-temperature torque method according to IP186. This test evaluates the extent to which grease retards the rotation of a slow-speed ball bearing by measuring starting and running torques at low temperatures. Behavior was investigated at -40, -54, -60, and -65 °C. Shown in Table 1, the starting torque is well below 1,000 N-mm at all temperatures, even at -65 °C. In contrast, the running torque of the PP grease is above 100 N-mm in all cases, showing that it does not drop substantially below the starting torque. Likely, the nanoparticle structure is stable against shear thinning at very low temperatures. Due to the presence of physically detached nanoparticles, flow properties of the PP grease will be largely unaffected by the glass transition temperature (Τg) of polypropylene, which is between -10 and -20 °C 14. This enables the use of this combination of nanoparticles and polypropylene at temperatures of -60 °C or even lower. Polypropylene polymer greases (without nanoparticles) based on a network microstructure will freeze below Τg and impair
- 45 NLGI SPOKESMAN, MARCH/APRIL 2018
low-temperature startup and running, as reported previously. Low application temperatures are also possible using lithium complex greases combined with low base oil viscosities. However, the trade-off is lower mechanical stability and reduced performance at intermediate and higher temperatures. 3.3. Bearing testing Figure 8 shows film building behavior of the PP greases during R2F testing at 80 °C and at low speeds in the range of 0 – 250 rpm. The calculated nominal film thickness is shown for reference, for PAO base oil of 68, 200, and 400 cSt viscosity at 40 °C, respectively. Comparison is made between film building of the PP grease after running-in for 100 h at 250 rpm, and after 176 h (7 days) of stop/start cycles. It can be seen that lubricant film formation is strongly enhanced compared to base oil lubrication. Also, with increasing speed, the film thickness becomes similar to the nominal film thickness for a base oil viscosity of approximately 200 cSt at 40 °C. The film-building properties are different directly after the running-in step and after completing the stop/start cycles. For the latter condition, the film thickness is finite even at very low speed, suggesting the PP thickener has formed a semi-permanent lubricant film. This behaviour is not seen after the running-in step. It is therefore feasible that the film formation is reversible depending on the operating conditions. In turn, this suggests that the interaction between the PP thickener and the bearing surface does not lead to a hard, solid film. The presence of a reversible film may be beneficial for reducing friction.
after 6 h, followed by a gradual and continuous temperature decrease to <45 °C after 48 h. The PP base grease and PP additized grease behaved similarly. At higher speeds, the self-induced temperature of the additized PP grease was consistently lower compared to the PP base grease. The latter showed a tendency to generate brief temperature peaks up to 80 °C, when ramping up the speed. In contrast the additized PP grease only showed minor temperature peaks when the speed was increased. Additional air cooling at 3,000 rpm (see experimental section) lowered the self-induced temperature by some 10 °C. At the highest speed of 4,000 rpm, temperatures reached approximately 67 °C for the base grease and 64 °C
Film thickness as measured after the running-in phase represents the lubricating conditions under steady state conditions. During stop/start cycles, the lubrication conditions will be interrupted, promoting grease migration and replenishment; it is likely that this triggers thickener interactions in the contact, leading to enhanced film formation even at very low speeds. The PP grease could be a preferred formulation for many application conditions where a selfadjusting lubricant film is beneficial. Figure 9 shows the self-induced temperature of the PP base grease and additized PP grease during R2F bearing testing at 1,000 – 4,000 rpm. The selfinduced temperature at 1,000 rpm reached a maximum of approximately 55 °C - 46 VOLUME 82, NUMBER 1
for the additized grease. Overall, the PP grease showed stable lubrication behavior, whereby additives lowered operating temperatures by 8 °C depending on speed and contributed to a smoother temperature profile. As discussed below, the presence of additives may suppress excess layer formation by the polypropylene, rather than providing an intrinsic friction reduction. Comparison of the additized PP grease, high-speed grease Li-III, and extreme pressure grease Li-IV, is shown in Figure 10. The self-induced temperature of Li-IV is consistently higher compared to that of the PP grease and Li-III. As Li-IV contains a mineral oil of higher viscosity (200 cSt at 40 °C), and has been optimized for high-load conditions, the observation of higher self-induced temperatures is not unexpected. Furthermore, bearing and grease analysis (below) show evidence of surface damage due to severe starvation effects at increasing speed (results not shown). This may also explain that the largest temperature difference (>10 °C) between the PP grease and Li-III is observed at the operating speed of 4,000 rpm. Li-III may be considered as a low-friction reference in the R2F testing, containing a low viscosity blend of PAO and synthetic ester (25 cSt at 40 °C). It can be seen that Li-III results in the lowest overall temperature at 4,000 rpm (58 °C), whereas the additized PP grease generates the lowest selfinduced temperature at 3,000 rpm. The overall temperature profile of both greases is surprisingly similar.
Synthesis of polymer grease is similar to that of porous polymeric materials, -, applying temperature-induced phase separation to a polymer-solvent mixture -. Here, typically a porous matrix with a lacy, cellular, or nodular morphology remains after solvent extraction . In this study, “porous polymer” is processed in the presence of its base oil “solvent” to obtain functional polymer grease. CryoSEM and TEM analysis show that after grease processing, the in-situ morphology consists of uniformly distributed, amorphous nanoparticles of 10–15 nm diameter, in the base oil. Van de Witte et al. extensively reviewed the experimental and theoretical research in understanding the mechanisms of formation of porous morphologies . Cooling a mixture of polypropylene and base oil leads to liquid-liquid phase separation; however, due to polypropylene solidification, this is essentially a solid-liquid phase separation process. The presence of nanoparticles indicates that, for the polymer grease, this occurs via nucleation and growth, as was shown previously for phase separation of polypropylene/mineral oil mixtures . It is likely that the copolymer used for polypropylene grease synthesis acts as a nucleating agent during nanoparticle formation. Therefore, the role of the copolymer could be critical in creating the microstructure. This behaviour is unlike the use of a copolymer as a modifier or co-thickener to improve, e.g., stability or oil separation properties. The properties of the polymer grease, when behaving as a nanofluid, will be governed by the interactions between particles and not by physical connections. Rheology shows that irreversible shear thinning does not occur; rather, the grease shows excellent stability and flow behaviour combined. This is also confirmed from the mechanical stability of the grease. Traditional polymer greases forming a network microstructure are inherently sensitive to mechanical degradation. The polymer grease also provides the basis for excellent lowtemperature flow behaviour, as it does not form a thickener network sensitive to solidification at low temperatures. This was confirmed in lowtemperature torque testing at temperatures as low as -65 °C. In this respect, previous polymer greases should not be compared with the new composition. It is commonly known that the grease thickener can enhance film formation in rolling contacts -. Recent studies correlate film thickness enhancement under fully flooded conditions to microstructure characteristics 
- 47 NLGI SPOKESMAN, MARCH/APRIL 2018
and predict increased thickener contribution with decreasing length scale of the microstructure . In our testing, the polymer thickener clearly enhances film formation, the extent of which is strongly dependent on speed and runningin conditions. We argue that deposition of polypropylene particles, carried by the base oil, results in enhanced yet reversible film formation. This may explain consistently low self-induced temperatures for the polymer grease, comparable to a high-speed lithium grease of lower base oil viscosity, over a wide speed range during bearing testing. We expect behaviour similar to that of a nanofluid close to the rolling contact, in a manner similar to that reported for nanoadditives in lubricants. Metallic, ceramic and mineral nanoparticles have been studied extensively for improving friction and wear characteristics of lubricating oils -. Notably, the ability of nanoadditives to penetrate and pass through the rolling contact during oil replenishment, thereby adhering or sintering at the surface, has been emphasized as the mechanism behind their performance. Polypropylene nanoparticles should be equally effective in reaching the surface, either by bulk grease or by oil replenishment, similar to nanoadditive behavior. This could lead to lubricant film enhancement and/or layer formation. A possible mechanism for friction reduction has been reported where spherical nanoparticles are flocculated and adhere to the rolling surface when trapped in the converging inlet gap of the lubricated contact . Polypropylene particle deposition may occur in a similar manner. This provides the conditions for the formation of very thin PP layers. In turn, this can contribute to friction reduction when associated with moderate layer formation. Generally, the lubricating film thickness in grease-lubricated bearings is determined by hydrodynamic action of the base oil under EHL conditions ; thus PP particles present will enhance base oil properties and/or boundary layer formation. Figure 11 shows a schematic representation of film thickness and pressure in a fully flooded and starved EHL contact . In the latter case, the film thickness is reduced at higher speeds due to a lack of lubricant in the inlet side of the contact. The change in thickness of these layers is given by the difference between the feed and loss flow rates of lubricant into or out of the raceways . It is expected that under fully flooded conditions of grease churning, the polymer grease acts as a highly concentrated nanofluid. This can lead to an imposed layer formation, and increased friction, due to the excess of thickener in the contact. When replenishment occurs due to oil bleeding from the bulk grease, particles will be diluted in the oil, and deposition in the contact will be greatly reduced. Under starved conditions, it can be expected that particles transported into the contact are effectively trapped, imposing thin layer
formation. It can be expected that layer formation continues under starved conditions provided oil replenishment occurs. In contrast, traditional greases rely on residual layers under starved conditions.
The polymer grease in this study consists of polypropylene nanoparticles uniformly distributed in base oil. A straightforward process leads to this structure: • Polymer grease preparation in a new two-step process of temperature-induced phase separation of a polypropylene polymer/PAO mixture, followed by processing at low-shear intensity. • Phase separation by nucleation and growth results in the formation of a network of connected polypropylene polymer nanoparticles. • The polypropylene polymer nanoparticles are spherical, solid and amorphous with a diameter of 10-15 nm. • Processing separates the particles from the network resulting in the formation of shear stable nanofluid. • The copolymer used is likely to act as a nucleating agent for nanoparticle formation. The polymer grease presented possesses some defining properties: • A high yield stress and fully reversible shear thinning behavior. • A thickener structure insensitive to mechanical degradation. • A stable grease consistency after prolonged shearing. • Enhanced lubricant film formation at low speed. This new generation polymer grease shows excellent lubrication performance: • The basic composition provides low friction performance over a wide speed range, similar to high-speed reference grease.
- 48 VOLUME 82, NUMBER 1
• Potential for use at extremely low start up temperatures, e.g., -65 °C without compromising the grease mechanical stability. • It is proposed that the polymer grease behaves as a nanofluid close to the contact, resulting in prompt release of oil and nanoparticles from grease into the rolling contact, whereas further away from the contact, grease settles and stabilizes.
The authors wish to thank Dr Stefan Lammens, Director of SKF Engineering and Research Centre, for his kind permission to publish this article.
1. NLGI: NLGI Lubricating Greases Guide. National Lubricating, Greases Institute, Kansas City, MO, 1994. 2. R. Mas, A. Magnin, “Rheology of colloidal suspensions-case of lubricating greases”, Journal of Rheology 38, 889–908, 1994. 3. M. A. Delgado, M. C. Sánchez, C. Valencia, J. M. Franco, C. Gallegos, “Relationship among microstructure, rheology and processing of a lithium lubricating grease”, Chemical Engineering Research and Design 83, 1085–1092, 2005. 4. M. A. Delgado, C. Valencia, M. C. Sánchez, J. M. Franco, C. Gallegos, “Influence of soap concentration and oil viscosity on the rheology and microstructure of lubricating greases”, Industrial Engineering Chemical Research 45, 1902–1910, 2006. 5. P. J. Shuff, L. J. Clarke, “Imaging of lubricating oil insolubles by electron-microscopy”, Tribology International 24, 381–387, 1991. 6. D. Meijer, B.O. Jacobson and H. Lankamp, “Polymer thickened lubricating grease”, Europe Patent 0700986, 28 July 1999. 7. D. Gonçalves, B. Graça, A.V.Campos, J.Seabra, J. Leckner, R. Westbroek “On the film thickness behaviour of PP greases at low and high speeds” Tribology International 90, 435 – 444, 2015. 8. T. Cousseau, B. Graça, A. Campos, J. Seabra, “Friction torque in grease lubricated thrust ball bearings”, Tribology International 44, 523-531, 2011. 9. D. Meijer, D. Muller, R. Thijssen, “Grease composition and method for making the same”, Europe Patent PCT/EP2015/080551 and WO/2016/102382, 30 June 2016. 10. J. L. Mansot, P. Terech, J. M. Martin, “Structural investigation of lubricating greases”, Colloids Surfaces 39, 321–333, 1989. 11. S. Hurley, P. Cann, “Examination of grease structure by SEM and AFM techniques”, NLGI Spokesman 65, 17–26, 2001. 12. P. J. Shuff and L. J. Clarke, “The structure of grease via electron microscopy and image analysis”, Lubrication Science 4(1), 35-50, 1991. 13. A. Margin and J.M. Piau, “Application of freeze-fracture technique for analyzing the structure of lubricant greases”, J. Mater. Res. 4(4), 990-995, 1989. 14. J. H. Gibbs and E. A. DiMarzio, “Nature of the Glass Transition and the Glassy State”, J. Chem. Phys. 28, 373-383,1958. 15. Nanoporous Polymers - Design and Applications, Vijjay I. Ramn and Giuseppe R. Palmese, in Nanomaterials Handbook, Yury Gogotsi (Editor), CRC Press, 2006, ISBN: 978-0-8493-2308-9. 16. M. Mulder and K. Dordrecht, Basic Principles of Membrane Technology, 1991, ISBN 0-7923-0978-2. 17. T. Tanaka and D. R. Lloyd, “Formation of poly(l-lactic acid) microfiltration membranes via thermally induced phase separation”, J. Membrane Sci. 238, 65–73, 2004. 18. F.J. Hua, T.G. Park, and D.S. Lee, “A facile preparation of highly interconnected macroporous poly(d,l-lactic acid-co-glycolic acid) (PLGA) scaffolds by liquid–liquid phase separation of a PLGA– dioxane–water ternary system”, Polymer 44, 1911–1920, 2003. 19. Theory and Examples of Spinodal Decomposition in a Variety of Materials, H.P.C. Schaftenaar, research paper, University of Utrecht depository, March 2008. 20. T.D. Li , L.M. Gan , C.H. Chew, W.K. Teo, L.H. Gan, “Preparation of Ultrafiltration Membranes by Direct Microemulsion Polymerization Using Polymerizable Surfactants”, Langmuir, 12(24), 5863–5868, 1996.
21. Thermodynamics of Polymer Solutions (MMI Press Polymer Monograph Series), Volume 1, Kurata, Michio, Harwood Academic Publishers, London and New York, 1982, ISBN 10: 3718600234. 22. Y.S. Nam, T.G. ParkY.S. Nam and T.G. Park, “Biodegradable polymeric microcellular foams by modied thermally induced phase separation method”, Biomaterials 20, 1783–1790, 1999. 23. A DSC-study on the demixing of binary polymer solutions, P.C vd Heijden, doctoral thesis, University of Twente, 2001. 24. P. van de Witte, P.J. Dijkstra, J.W.A. van den Berg, J. Feijen, “Phase separation in polymer solutions in relation to membrane formation”, Journal of Membrane Science 117, 1-31, 1996. 25. D.R. Lloyd, K.E. Kinzer and H.S. Tseng, “Microporous membrane formation via thermally induced phase separation. I. Solid-Liquid phase separation”, Journal of Membrane Science 52, 239-261, 1990. 26. D.R. Lloyd, K.E. Kinzer and H.S. Tseng, “Microporous membrane formation via thermally induced phase separation. II. Liquidliquid phase separation”, Journal of Membrane Science 64, 1-11, 1991. 27. I. Corroné, P. Vergne, D. Mazuyer, N. Truong-Dinh and D. Girodin, Effects of grease composition and structure on film thickness in rolling contacts, Tribology Transactions 46, 31-36, 2003. 28. A. R. Wilson, The relative thickness of grease and oil films in rolling bearings, Proceedings of the Institution of Mechanical Engineers 193(17), 185-192, 1979. 29. P. M. Cann, “Grease lubrication of rolling element bearings—role of the grease thickener”, Lubrication Science 19(3), 183–196, 2007. 30. P. M. Cann, A. A. Lubrecht, “An analysis of the mechanisms of grease lubrication in rolling element bearings”, Lubrication Science 11(3), 227–245, 1999. 31. H. Åström, J. O. Östensen, E. Höglund, Lubricating grease replenishment in an Elastohydrodymanic point contact, J. Tribol. 115(3), 501-506, 1993. 32. W. S. Zhu, N. Y. Neng, A theoretical and experimental study of EHL lubricated with grease, J. Tribol. 110(1), 38-43, 1988. 33. P. M. Cann, B. P. Williamson, R. C. Coy, H. A. Spikes, H.A., “The behaviour of greases in elastohydrodynamic contacts”, Journal of Physics D Applied Physics, 25(1A), 124–132, 1992. 34. P. M. Cann, H. A. MSpikes, “Film thickness measurements of lubricating greases under normally starved conditions”, NLGI Spokesmen 56(2), 21–27, 1992. 35. P.M. Cann, “Starvation and reflow in a grease-lubricated elastohydrodynamic Contact”, Tribology Transactions 39(3), 698–704 (1996). 36. M. Kaneta, T. Ogata, Y. Takubo, M. Naka, “Effects of a thickener structure on grease elastohydrodynamic lubrication films”, Proceedings Institutional of Mechanical Engineers, Part of Journal of Engineering Tribology 214(4), 327–336, 2000. 37. F . Cyriac, P. M. Lugt, R. Bosman, C. J. Padberg, C. H. Venner, Effect of Thickener Particle Geometry and Concentration on the Grease EHL Film Thickness at Medium Speeds, Tribology Letters 61:18, 2016. 38. A . H. Battez, R. González, J. L. Viesca, J. E. Feranández, J. M. Díaz Fernández, A. Machado, R. Chou, J. Riba, “CuO,ZrO2 and ZnO nanoparticlesas antiwear additive in oil lubricants”, Wear 265, 422–428, 2008. 39. Y . Y. Wu, W. C. Tsui, T. C. Liu, “Experimental analysis of tribological properties of lubricating oils with nanoparticle additives”, Wear 262, 819–825, 2007. 40. M . Zhang, X. B. Wang, X. S. Fu, Y. Q. Xia, “Performance and antiwear mechanism of CaCO3 nanoparticles as a green additive in poly-alpha-olefin”, Tribolology International. 42, 1029–1039, 2009. 41. F . Chinas-Castillo & H. A. Spikes, “The Behavior of Colloidal Solid Particles in Elastohydrodynamic Contacts” , Tribology Transactions, 43:3, 387-394, 2000 42. M .T. van Zoelen.Thin layer flow in rolling element bearings. PhD thesis, University of Twente, the Netherlands, ISBN 978-90-3652934-1, December 2010. 43. V . Wikström and B. Jacobson. Loss of lubricant from oil-lubricated nearstarved spherical roller bearings. Proceedings of the Institution of Mechanical Engineers. Part J: Journal of Engineering Tribology 21(1):51–55, 1997.
Lubricating Grease Thickeners: How to Navigate your Way through the Lithium Crisis By: Gareth Fish, PhD CLS CLGS, Chris Hsu, PhD, and Robert Dura, PhD The Lubrizol Corporation Abstract The most important difference between a lubricating grease and a liquid lubricant is the thickener that gives the grease its structure. The thickener is responsible for the non-Newtonian behavior and some characteristics of the lubricating grease. Since Clarence E. Earle first filed for a US patent in 1940 for the use of lithium soaps as lubricating grease thickeners, their use has grown to 75% of the global market. Grease makers are looking to replace, supplement or change the lithium and lithium complex thickener systems of greases that they manufacture with alternative thickeners due to critical changes in cost and availability of lithium. This paper will review the 2015 NLGI grease production survey, discuss thickener options, and highlight experimental results for three thickener systems that deliver the same performance as lithium. These three thickener options are borate ester technology, anhydrous lithium hydroxide dispersions, and high soap calcium sulfonate complexes. Introduction The largest volume of grease thickeners sold globally are lithium soaps with around 54.5% based on conventional soaps and lithium complexes at almost 20% of the global market in 2015 (1). Comparing these volumes to the 2005 figures (2), it is apparent that the volume of simple lithium soap has fallen from 57.6% to 54.5%, but the volume of lithium complex thickeners has almost doubled from 10.8% to 19.7%. This is a significant simplification of the actual regional volumes, and to understand the need for alternative thickener technology these volumes need to be looked at regionally. • In North America, lithium complex thickeners are the dominant player with 39.1% of the market followed by conventional lithium soaps (25.8%) and aluminum complexes being a distant third (8.8%). All calcium soaps grouped together make up only 4.5% of the market
• In Europe, conventional lithium soaps make up 53.3% of the market, lithium complex thickeners 16.3%, and no other thickener more than 6%. Collectively though, calcium soap greases make up just over 10% of the market. • The other significant regional differences are Japan and the Indian Sub-continent. In Japan, 56.4% of thickeners is conventional lithium soap, but only 3.1% s lithium complex. The other commonly used thickener volumes are polyurea and urea complex with 28% of the market. Calcium soaps and other specialty thickeners account for around 5% each. By contrast, in India, conventional lithium soaps dominate the market approaching 85% with complexes only around 7%. The Chinese market consists of 63.6% conventional lithium and 16.9% lithium complex thickeners. The rest of the world uses approximately 150,000 metric tons (12.3% of the global grease volume); about 53% is conventional lithium and 20% lithium complex. A conventional lithium grease thickened with only 12-hydroxystearic acid uses about 1.2 wt% of lithium hydroxide monohydrate (LHM), and a diacid carboxylate complex grease uses about 2.0 wt% LHM. Reviewing grease volumes, it is clear that the growing volume is lithium complex with conventional lithium embracing the commodity market. There is a perceived need to improve the properties of lithium complex greases in the following areas: water resistance; oxidation stability, grease life; and bleed. Oxidation stability and life improvements have been presented previously (3), and polymer technologies are available to improve water resistance (4). In North America, new specifications have appeared that require dropping points above 280 °C. Some customers have requested thickener systems that have consistently high dropping points above 300 °C, trying to match the behavior of calcium sulfonate greases. However, the majority of lithium complex greases sold in North America have dropping points
- 50 VOLUME 82, NUMBER 1
of 260 째C to 280 째C. Historically in Europe, higher temperature greases had to possess dropping points only above 220 째C. With the globalization of specifications, dropping points for high temperature greases above 260 째C are now required by the majority of published specifications. In the last 10 years, lithium ion batteries have risen to be the energy storage media of choice. The battery in a cell phone uses up to 6 grams of lithium, whilst a laptop computer or tablet uses 20 to 40 grams of lithium (5). The biggest new drivers of lithium demand are plug-in electric vehicles. It is estimated that a 70 kWh battery to power a plug-in electric bus or performance car would use 63,000 grams of lithium, the equivalent to 10,000 cell phones. From Table 1, the amount of lithium metal used in grease in 2015 was around 2,000 metric tons. The volume of lithium metal sold into batteries in 2015 was 12,000 metric tons. This volume is predicted to increase to 24,800 metric tons in 2020 and to 48,700 metric tons in 2025. This volume for batteries is larger than the projected supply volume available (5). This demand for lithium for batteries has created a shortage of supply and a significant increase in prices of LHM. In 2016, the price of LHM doubled in North America, tripled in most of the rest of the world, and in India rose more than seven times the average 2015 price. For a conventional lithium grease in North America, the cost of LHM increases the cost of the base grease by about 13% and by about 19%.for a carboxylate lithium complex base grease. Grease makers are now looking to replace, supplement or change the lithium and lithium complex thickener systems of greases that they manufacture with alternative thickeners. Reviewing the available options for grease makers it is clear that the usable alternative thickeners depend on significant regional market forces and manufactured volumes. This paper will now discuss thickener options and highlight a few ways that grease makers can deliver the same performance with modified and alternative thickener systems.
Industrial and Automotive Grease Options In North America, lithium complex is the dominant thickener with conventional lithium soaps being mostly used for commodity greases. A significant portion of the lithium complex greases is used in automotive applications. Today, very little calcium sulfonate, aluminum complex or calcium sulfonate complexes are sold into the automotive industry. Based on past experiences, it is not likely that the volumes of these three thickener types will increase much for automotive applications. It should be possible for North American automotive component manufacturers to migrate to urea thickened greases like those used in the Japanese automotive industry. In Japan, there appears to be available capacity to manufacture urea greases, and it is likely that the migration to urea greases from lithium will further accelerate in Japan. For industrial applications, lithium complex greases, can be replaced by calcium sulfonate, aluminum complex or calcium sulfonate complexes and in some instances, where compatibility is not an issue, by clay thickened greases. Electric motors are another area where both lithium complex and urea thickeners are used. Prior to the recent steep rise in lithium prices, lithium complex greases were a lower cost option for electric motors compare to the higher priced ureathickened greases. The gap in costs has narrowed, and lithium complex grease prices may rise above those for urea greases if the LHM price rises much further. In Europe, the outlook appears to be much bleaker. Chemical regulation of di-isocyanates and urea thickeners seems to preclude switching to urea greases. Again, the European automotive industry has little experience using calcium sulfonate and aluminum complex greases. For industrial greases, these two thickeners would offer alternatives, as would using anhydrous calcium, clay, or calcium complex thickeners, which are still made in quantity. However, calcium greases do not match the temperature profile of lithium greases, and it would be necessary to improve the thermal stability of calcium
- 51 NLGI SPOKESMAN, MARCH/APRIL 2018
grease in order to replace lithium grease. In India, grease makers face similar challenges to their colleagues in Europe. They have been looking to replace lithium greases with mixed calcium-lithium soap (6) for automotive applications, but face the thermal stability issue of calcium and mixed soap greases. Titanium complex greases have been proposed for steel mills and other industrial uses (7). Work has just started in India to look at urea greases (8) for use as alternatives to lithium complex greases. The use of boron additives in lithium greases Boric acid has been used for a number of years as an alternative to aromatic acids or dicarboxylic acid complexing agents for lithium greases. As described in the NLGI Grease Guide 6th Edition (9), boric acid can be difficult to incorporate and is currently the subject of regulatory scrutiny. Other sources of boron that can be more easily incorporated into the greases are now preferred. Borate esters are a relatively easy way to deliver higher dropping points. Traditionally, low molecular weight borate esters were used, but other components to do this are now available. Lorimor (10) described and reviewed various boron chemistries that are available, noting that some work better when used in conjunction with a zinc dithiophosphate (ZnDTP) additive. Table 2 compares data for several combinations of borate and ZnDTP additives in a lithium base grease. Based on the data presented in Table 2, borate esters can deliver elevated dropping points. However, borate esters are not without issue. Hydrolytic and thermal stability can be poor and they can release alcohols and boric acid, which is an
environmental concern in some markets. The alcohols can give rise to odors, which may be undesirable. The earliest borate esters used butanol or isobutanol. Because of the issues related to hydrolytic and to thermal stability, along with the pungent odors, additive manufacturers switched to longer chain alcohols for the products sold today. A new lower odor borate ester was developed and tested in a variety of greases to investigate its effect on the dropping points and to explore its use as a grease complexing agent. The first study used a conventional lithium grease base with an ISO VG 100 Group I mineral oil and compared two borate esters, with and without ZnDTP. The current borate ester was BE1, and the new, lower odor borate ester was BE2. The base greases were heated to 100 Â°C and the borate esters were mixed in, followed by the ZnDTP. Then, the greases were milled and de-aerated. As can be seen from the data in Table 3, the new odorless borate ester (BE2) additive matched the behavior of the current borate ester (BE1). All greases treated with the borate esters had dropping points above 260 Â°C. Grease complexing agent issues The demand for lithium complex grease has increased globally by 30% over the last few years, from 15% of the market in 2005 to just under 20% in 2015. Typical dicarboxylate lithium complex greases use around 2.0% lithium hydroxide compared to around 1.2% for a simple lithium grease or a borated lithium complex. According to the NLGI Grease Guide (9), a complex soap thickener contains a thickening soap and a complexing agent. The thickening soap solidifies the base oil, and the complexing agent gives the thickening soap better thermal stability. The Guide further states that the choice of complexing agent depends on the metal in the thickening soap. Calcium soaps are typically complexed with acetic acid, and aluminum soaps are complexed with benzoic acid. The first complexing agent used for lithium soaps was acetic acid (9), but this did not give the grease the same stability as it did for calcium greases. In the 1970s, boric acid was first used as a complexing agent. Other aromatic organic acids such as salicylic or
- 52 VOLUME 82, NUMBER 1
p-hydroxybenzoic acid were also first used about this time, but today only a small number of manufacturers still use this technology. Dicarboxylic acids became the complexing agents of choice and dropping points above 260 Â°C could be readily obtained. At the current time, azelaic (C9) and sebacic (C10) acids are used most commonly, and adipic (C6) and dodecanedioic (C12) are used to a lesser extent. As reported in 2014 (11), it can be challenging to control the grease making process to get good complexing with these acids. Today there appears to be a supply shortage of sebacic acid, which is further restricting the growth of lithium complex greases. In their 2014 NLGI paper, Fish and Hsu (12) outlined how the use of a micronized and dehydrated lithium hydroxide dispersion in oil could help to make superior carboxylate lithium complex greases with higher dropping points and better thermal stability. With todayâ€™s issues related to the cost and supply instability of LHM, that work was revisited and looked at not from a view point of making the grease better, but to match the performance at lower lithium and complexing acid content. Four greases (358, 365, 366 and 375) were compared. Greases 358 and 375 used the same amount of 12-hydroxystearic and azelaic acids (73.8 and 22.9 g, respectively), as did Greases 365 and 366 (86.3 and 10.7 g, respectively) but different amounts of lithium hydroxide additives and base oil, Table 4. The amount of oil for the lithium dispersion greases was reduced to keep the thickener content constant and was targeted at 10 wt% thickener. It was reported that the lithium hydroxide dispersion not only reacted faster and reduced the time to process a batch, but also gave slightly better grease yields (12). However, comparing the raw material costs of greases 358 and 375, the one using the lithium hydroxide dispersion (358) on an equal cost basis attracts
about a 3% premium over the cost of the one manufactured with LHM in water (375). Comparing the penetrations and dropping point of Grease 375 with Grease 365, these basic properties are the same (within test method repeatability). Comparing the raw material costs for greases 365 and 375), the one using the lithium hydroxide dispersion with the lower content of diacid (grease 365), offers a cost reduction of 5.5% compared to the cost of the grease made with standard LHM powder mixed with water route (grease 375),. The additional thing to note from the previous paper is that it takes about 4 hours less to run a 1 step process with a single co-saponification reaction compared to running a two-step sequential saponification. The data for the four carboxylate complexes is included in Table 4. Not only does the use of the lithium hydroxide dispersion use less diacid, but also saves considerably on the amount of lithium equivalents needed for each batch of grease. Borate esters as complexing agents As reported earlier, boric acid is a well-known complexing agent for lithium greases but is not without issues. The key question that has arisen about the use of borate esters in grease is whether they can replace both boric acid and dicarboxylic acids as complexing agents. To address this question, three greases were prepared. The base oil was a mixture of 112 mm2/s (112 cSt at 40 Â°C) Group I paraffinic oil and 2000 Dalton (g/mol) polyisobutylene (PIB), giving an ISO VG 220 final base oil viscosity. All three greases used the same multi-purpose zinc-containing additive package at 4% treat rate. This additive package was used in order to
Notes: Penetration is defined as the distance a cone of specified dimensions, mass and surface finish falls into the grease when allowed to drop for 5 seconds. The penetration is measured in tenths of a millimeter, typically written as dmm (9). Thickener concentration calculation is given in the Appendix. - 53 NLGI SPOKESMAN, MARCH/APRIL 2018
compare the influence of the thickener on the performance of finished grease. The first sample, Grease 89, was a 2:1 acid mole ratio sebacate complex with a thickener content of 10.7 wt%. The second, Grease 90, was a conventional lithium soap grease with 5.5 wt% 12-hydroxystearate soap, and the third, Grease 91, had 5.7 wt% lithium 12-hydroxystearate soap complexed with 2 wt% of the low odor borate ester, BE2. Standard tests were carried out to compare the performance of these three greases and the results are reported in Table 5.
The data gathered so far show that a borate ester lithium complex grease performs as well as a dicarboxylate lithium complex and better than a conventional lithium soap grease. The increase in oxidation life for the borate grease, measured by the increase in oxidation induction time (OIT) using pressure differential scanning calorimetry (PDSC), confirmed results reported by Lorimor (10). Also revisited were the rheological behaviour and a reciprocating temperature ramp test used by Lorimor (10). In this rheology test, the lithium soap grease started to soften above 180 °C, but the two complex greases were fairly stable to 260 °C. The behaviour of the three greases is shown in Figure 1. By switching from a diacid to a borate ester for the complexing agent, grease makers can save on the raw material costs for making a lithium complex grease. Looking at just raw material costs for conventional lithium and borate esterlithium complexes, based on the current price of LHM ($25 / kg) it still just cost effective to use it as the lithium source. Moving to the borate ester complex would use significantly less LHM and, in the case of supply shortage, allow the grease maker to produce 2.7 times the amount of borate ester-lithium complex grease compared to a dicarboxylate complex. Comparison of the costs of the grease and the amounts of LMH and lithium metal are included in Table 6. The use of borate ester additives in calcium greases The next option studied to reduce the reliance on lithium hydroxide was to investigate if anhydrous calcium greases could be used instead of lithium soap greases. In North America, anhydrous calcium greases account for about 3.8% of the market, which equates to 8,300 metric tons. In China, 14,000 metric tons of anhydrous calcium soap greases are sold (3.5% of the market), and in Europe, the volumes are 3.2% of the market or 6.500 metric tons. If the ISO 2176 or IP 396 test methods are used to measure the dropping point of anhydrous calcium greases, a typical value of around 145 °C is obtained.
When using the ASTM D2265 method, dropping point values of around 155 °C are obtained. This latter test method is not used widely in Europe. Several specifications demand a dropping point above either 163 °C or above 177 °C, which cannot be met easily by anhydrous calcium greases, and hence, conventional lithium soap greases are used. The present study investigated whether borate ester chemistry could boost the dropping point of such anhydrous calcium greases, with and without ZnDTP, to above the 163 °C minimum requirement. An NLGI #2 anhydrous calcium soap grease was prepared using an in situ reaction of hydrated lime mixed with water and 12-hydroxystearic acid in a 30:70 blend of a 750 naphthenic oil with a Group II 600N paraffinic oil. Table 7 shows the data from the study of borates on the dropping point of anhydrous calcium greases. The results of this study showed that it was possible to use borate esters to achieve dropping points above 163 °C but not above the 177 °C minimum. This suggests that borate esters
could be used to boost the dropping point to meet some lower lithium soap specifications but not applications that required dropping points above 177 °C. Next, this study investigated the use of borate esters to increase the temperature resistance of mixed soap calciumlithium greases and check whether they could exceed the 177 °C limit. Initially, an anhydrous calcium grease (C6) and a conventional lithium grease (L11) were manufactured using the same naphthenic-paraffinic base oil blend from above. Dropping points were measured after these greases were manufactured and again after treating with 3 wt% of the borate ester BE2 as above. Samples of the two base greases (C6 and L11) were then combined in ratios of 75:25, 50:50 and 25:75. The samples were milled and deaerated and tested for dropping point, and then treated with 3 wt% of the borate ester BE2 and tested. The dropping point results in Table 7 for the simple mixtures did not reach the target of 177 °C without mixing more than 50 wt% of the lithium soap base mixed with the anhydrous calcium base.
- 55 NLGI SPOKESMAN, MARCH/APRIL 2018
However, mixing a finished lithium 12-hydroxystrearate grease and with an anhydrous calcium grease is not a practical reality. Three new greases were manufactured in the same base oil blend as before. The 12-hydroxystearic acid was heated in the oil, and then the lime and lithium hydroxide monohydrate (mixed together with water) were added to the oil. The mixture was held at 90 °C or one hour for saponification and then heated to 200 °C followed by cooling to 100 °C. Each sample was then divided in two equal portions, and borate ester BE2 was added to one portion. The greases were milled and deaerated, and dropping points were measured by ASTM D2265, Table 9. It is clear from the dropping point data in Table 9 that adding 3 wt% of the BE2 to the 75 wt% calcium: 25 wt% lithium mixed soap grease (Grease MS10) gave a similar dropping point (187 °C) to that of the 25 wt% calcium: 75 wt% lithium (Grease MS9) without the borate ester (189 °C). Both MS9 and MS10 had higher dropping points than the177 °C target. With the borate ester, it was possible to use a lower amount of lithium grease to meet this dropping point specification. The next step was to look at the relative costs of using additional lithium hydroxide versus adding the borate ester. Raw material costs were calculated from typical market prices for hydrated lime, LHM, 12-hydroxystearic acid, and the two base oils. Relative costs for the various options could be compared on a raw material basis, normalized to the cost of one kilogram of the anhydrous calcium soap thickened grease,
C6. The relative costs in Table 10 illustrate that at June 2017 prices of LHM, there is almost no cost difference between MS9 and MS10 greases. The biggest difference is that MS10 uses one third of the amount of LHM compared to MS9. If the price of LHM rises (and/or its availability becomes limited), a formulation such as MS10 becomes more attractive. Calcium Sulfonate Greases Sulfonate greases have found widespread use in applications that require high temperature tolerance and good load carrying capacity. The general process for making gelled calcium sulfonate grease has remained largely unchanged since these types of greases were first developed in the 1960s (13). Firstly, an overbased calcium sulfonate with a total base number (TBN) of 300 to 500 mg KOH / g equivalents is added to a grease kettle. The highly overbased sulfonate is mixed with base oil and treated with acid to destabilize the micellular structure. Then, promoters and water are added, and the material is heated to its gelation temperature. Provided that the water and promoters are retained in the mixture, the amorphous calcium carbonate is converted to crystalline calcite within one to five hours. The final step is the removal of water and promoters from the mixture. Prior to 1985, calcium sulfonate greases based on natural sulfonates (a by-product of Group I refining in which the distillate fraction is treated with oleum to remove aromatics) were a niche product manufactured and sold only in small quantities. The greases had very good antiwear and extreme pressure (EP) properties without the use of additives along
- 56 VOLUME 82, NUMBER 1
with dropping points above 300 °C and low oil separation. Their negative aspects were high thickener content and associated cost compared to other greases, and water spray off and low temperature mobility. At the NLGI Annual Meeting in 2008, Denis and Sivik (14) presented a paper on improvements to calcium sulfonate gelling technology. They outlined a procedure to incorporate the promoter system into an overbased synthetic sulfonate so that only base oil and water were needed for gelation. This procedure avoided issues associated with ‘flash’ of isopropanol and other alcohols used in gelation. Their work opened up the potential for sulfonate grease technology to a wider number of grease makers. However, this process did not produce grease faster than other sulfonates. One further challenge with calcium sulfonate technology is the promoter, an azeotrope mixture of alcohol / glycol, and water. If gelation is not carried out in a closed reactor, promoter and water are lost, and the gelation reaction stalls. At 90 °C, this loss of promoter and water takes between 60 minutes and 90 minutes. Carrying out the gelation at a colder temperature (80 °C) slowed down both the calcite conversion and the loss of promoter, no improvement in process time, and no prevention of stalling. In the present study, two possible avenues were explored to try to make the gelation process faster and more user friendly. The first avenue explored was to change the alcohol/glycol promoter. In earlier work (14), isopropanol worked well as did hexylene glycol. Propylene glycol, which is approved as a promoter for food grade greases, did not work when used at equivalent hydroxy content and equivalent weight. Other promoters, including 2-methoxyethanol and mixtures of alcohols and glycols, did not improve the processing time to gel the grease faster than the original alcohol/glycol promoter.
The second area of investigation was to change the acid. The current process uses an alkenyl-substituted carboxylic acid, a fairly weak organic acid. Succinic and sulfonic acids are used according to some of the published literature. (13), (14), and (15). Mixtures of succinic acid with alkyl-substitutions were tried as well. Short chain succinic acids generally produced firmer gels with higher yields than long chain succinic acids, but the amount of time to gel was the same. Unsubstituted succinic acid had to be melted and dissolved into the oil prior to reaction, which made it more difficult to handle them than the substituted succinic acids, which were viscous liquids at room temperature. Succinic anhydride was also tried, but it was necessary to hydrate it before use. The logarithmic acidity constant (pKa) of acetic (4.8), succinic (4.3), and alkyl-substituted succinic acids (5.6) identifies them as weak acids. These weak acids react more slowly with weak bases than stronger acids with a pKa < -2. Sulfonic acids can have pKa values down to -2.8, and the reaction with the lime can proceed very quickly in some cases. This results in a faster destabilization of the micellular structure of the sulfonate and faster conversion. Therefore, a commonly used alkylbenzene sulfonic acid was chosen to replace the alkylsuccinic acid. A series of sulfonate blends was prepared with different ratios of the acids to sulfonates and to the glycol/alcohol. Speed of gelling, ease of use, and basic properties of the gels were investigated. A particular acid ratio was chosen for scale up because it produced much faster gelling than the previously reported 3 hours (14). A batch of grease made with 63% of the new sulfonate blend and 37% of BS150 oil was made in under two hours from start to finish. The basic properties of this grease are in Table 11.
- 57 NLGI SPOKESMAN, MARCH/APRIL 2018
Calcium sulfonate complex greases In 1985, Muir and Blokhuis (16) were granted US Patent 4,560,489 disclosing a calcium sulfonate complex grease that used boric acid and 12-hydroxystearic acid in the process. In the patent narrative, the sulfonate was described as being made from a natural sulfonate, and the water washout was reported as being similar to other greases. Subsequent work by Barnes (15) used synthetic rather than natural sulfonates and swapped out the boric acid for phosphoric acid. Both patents described a two-step process of gelation followed by saponification. Olsen et al. (17) reported a further development of a one-step process to make calcium sulfonate complex greases by adding the acids with the lime. Typical data for gelled calcium sulfonate, calcium sulfonate complex, and lithium complex thickener (without added polymer) greases with a similar oil blend are compared in Table 12. The sulfonate complex data in Table 12 were as reported by Barnes (15) and not independently verified. Calcium sulfonate complexes have been historically sold as premium products offering good general properties and performance. The calcium sulfonate grease reported by Denis (14) is very much a premium product with excellent properties and has a much higher cost position compared to the two complex greases. The calcium sulfonate complex reported by Olsen et al (17) would be termed a high sulfonate - low soap complex. As the amount of soap in a grease is increased and the amount of sulfonate and calcite is reduced, the load carrying capacity of the grease decreases and the grease becomes less resistant to spray off. By moving to a low sulfonate - high soap grease, it should be possible to match the basic properties of lithium grease.
Acetic acid is used in many sulfonate grease making processes (15), (16) especially when the starting overbased calcium sulfonate has a high direct base number (DBN), which equates to the amount of “free” lime. One upside of using higher DBN sulfonates that require acetic acid for gelation is that they produce calcium acetate, which is well known to boost the Timken OK load. For some grease makers, it is not possible or desirable to use acetic acid, and so alternative acids are needed. If the grease has a lower amount of “free” lime, then it is typically easier to gel. As indicated earlier, there are issues in some markets with boric acids, and it is now preferable to avoid using them in sulfonate complex greases. Phosphoric acid, as per Barnes (15), can be used to make calcium phosphate in situ, or alternatively, calcium phosphate can be added as a powder or as calcium hydroxy apatite (18). Synthetic linear alkylbenzene (LAB) sulfonates are typically the lowest cost position, and by using this as the sulfonate, along with a high level of calcium soaps, greases can be prepared to match the performance and cost of lithium complex greases. Calcium sulfonates used for grease are typically 400 TBN with DBN values of around 40 mg KOH / g eq. Additionally, 300 TBN calcium sulfonates, with DBN values from 30 mg KOH / g eq. to 40 mg KOH / g eq. can be used, but the process is more challenging. In order to determine the cost and performance benefits of calcium sulfonate complexes and how they compare, three greases were manufactured with the same paraffinic brightstock (BS150) base oil, synthetic linear alkylbenzene sulfonate, dodecylbenzene sulfonic (DDBSA) and 12-hydroxystearic acids, glycol, lime and water. The formulations are listed in Table 13.
- 58 VOLUME 82, NUMBER 1
The three greases were then compared with standard property testing. As expected, the standard sulfonate performed better overall than the complexes, but at a higher raw material cost. These data show that the low sulfonate complex grease behaved similarly to an additized typical lithium complex grease. Summary and Conclusions This paper has shown that there are now several different routes available to help the grease producer to overcome the current cost and supply issues with lithium hydroxide monohydrate. The routes discussed were: manufacture greases with borate ester technology to reduce the amount of lithium; use anhydrous lithium hydroxide dispersions as alternative lithium sources; and offer high soap calcium sulfonate complexes. In this study, all three routes were used successfully to achieve performance comparable to standard lithium and
lithium complex greases. Acknowledgements The authors wish to acknowledge many co-workers and departments within The Lubrizol Corporation for their contributions to this work. References (1) Grease Production Survey Report 2015, NLGI, Lee’s Summit, Missouri 64063 (www.NLGI.org) (2) Grease Production Survey Report 2005, NLGI, Lee’s Summit, Missouri 64063 (www.NLGI.org) (3) Ward, Jr., W. C., and Fish, G., “Development of Greases with Extended Grease and Bearing Life Using Pressure Differential Scanning Calorimetry and Wheel Bearing Life Testing.” NLGI Spokesman 2010 V74(5) pages 14-27
- 59 NLGI SPOKESMAN, MARCH/APRIL 2018
(4) Ward, Jr., W. C., and Qureshi, F.S. “Influence of components blended to a target base oil viscosity on liquid phase and lithium grease properties” NLGI Spokesman 2009 V74 (1) pages 21-31 (5) http://www.dakotaminerals.com.au/index.php/lithium/ about-lithium (6) Goyal, A.K., Parameshwaran, N., Ghosh, B., and Sengupta, A. “Development of Advanced Calcium-Lithium Soap Grease with Minimum Uses of Lithium Hydroxide”, 18th NLGI India Annual Meeting, Aamby Valley City, Lonavala, Maharashtra, February 2016 (7) Mazumdar, S. “Superior Performance of Titanium Complex EP Grease in Steel Plant Applications – A Case Study” 18th NLGI India Annual Meeting, Aamby Valley City, Lonavala, Maharashtra, February 2016 (8) Deshmukh, V. “Polyurea Grease – An Ideal Cost Effective Replacement for Lithium Complex Grease for Automotive and Industrial Applications” 19th NLGI India Annual Meeting, Varanasi, Uttar Pradesh, February 2017 (9) NLGI Grease Guide, 6th Edition, 2015 NLGI, Lee’s Summit, Missouri 64063 (www.NLGI.org) (10) Lorimor, J.J., “Improving the Heat Resistance of Simple Lithium Soaps Using Borated Additives”, paper #0912, 77th NLGI Annual Meeting, Bonita Springs, FL, June 2010 (11) Morgan, D., Kay, J.S. and Coe, C., “Critical Variables in Lithium Complex Grease Manufacturing” paper #1313, 80th NLGI Annual General Meeting, Tucson, Arizona, 2013 (12) Fish, G. and Hsu, C., “Technology to Improve the Grease Making Process” paper #1422, NLGI 81st Annual Meeting, PGA National Resort, Palm Beach Gardens, Florida, June, 2014 (13) McMillen, R.L., “Basic Metal-Containing Thickened Oil Compositions,” US Patent 3,242,079 USPTO March 22, 1966 (14) D enis, R.A and Sivik, M. R., “Calcium Sulfonate GreaseMaking Processes,” paper #0812, NLGI 75th Annual Meeting, Williamsburg, Virginia, June, 2008 (15) B arnes, J. NCH Corporation, “Calcium Sulfonate Grease and Method of Manufacture”, U.S. Patent 5,126,062 USPTO June 30, 1992. (16) M uir, R.J. and Blokhuis, W., “High Performance Calcium Borate Modified Overbased Calcium Sulfonate Complex Greases,” US patent 4,560,489 USPTO December 24, 1985 (17) Olsen, W.D., Muir, R.J., Eliades, T.I., and Steib, T., Witco Corporation “Sulfonate Greases”, U.S. Patent 5,308,514 USPTO May 3, 1994. (18) Waynick, J.A., “Calcium Sulfonate Complex Greases Using Calcium Hydroxyapatite as a Hydroxide-Containing Basic Reactant” Paper #1508 NLGI 82nd Annual Meeting, Coeur d’Alene, Idaho, June, 2015
Appendix Calculation of Thickener Content Soap Concentration Calculation 1) Determine the saponification number (Sap#) and molecular weight (Mw) for each acid. Sap# = 56110 x MolWt x n where 56110 is the number of milligrams in one gram-molecular weight of KOH and n is the number of KOH molecules that react with one acid molecule For 12-hydroxystearic acid (12HSA), Sap# is normally about 188, Mw is 300.483 g/mol, and n=1 For Azelaic acid (AA), Sap# is normally about 590. Mw = 188.22 g/mol, and n=2. 2) Then determine the number of equivalents (eq) Equivalents (moles) = grams/Mw Total up the number of acid equivalents Total acid eq = Eq12HSA + EqAA 3) D etermine the % LiOH in the lithium source and the number of base equivalents 4) S ubtract the acid eq from the base eq and from this determine the amount of free LiOH (grams) 5) Calculate the amount of each soap assuming 100% conversion Lithium 12-hydroxystearate (g) = Eq12HS*(Mw12HSA – 1.008 +6.94) where MwLi12HS = Mw12HSA – MwH + MwLi Dilithium azelate (g) = (EqAA/2)*(MwAA- 2.016+13.88) and MwLi2AA = MwAA – 2MwH + 2MwLi Free LiOH (grams) = Excess EqLi*23.94 6) Sum these three gram weights = amount of thickener (grams) 7) Add up the total amount of grease made % thickener = mass of thickener (g) / mass of grease (g) Acid ratio calculator Moles Number of fatty acid moles: Number of complexing acid moles Equivalents Number of fatty acid equivalents: Number of complexing acid equivalents Worked example (5 kg of grease) 440 g 12-Hydroxystearic acid 1.474 moles = 1.474 equivalents 139 g Azelaic acid 0.737 moles = 1.474 equivalents 128 g LMH 3.056 moles = 3.056 equivalents 4400 g base oil Makes 600 g soap 2:1 molar acid ratio 12.0% thickener by weight
- 60 VOLUME 82, NUMBER 1
WE’VE GOT A GREASE FOR THAT
TREAT YOUR BRAND LIKE A KINGTM PARTNER WITH AN EXPERT IN OIL & GREASE PRIVATE LABEL MANUFACTURING We know exactly what independent lubricant manufactures need — because we are one. Take advantage of our century of experience, custom formulation expertise, and production capacity of 50 million pounds of grease and 20 million gallons of oil, annually.
CALL OR EMAIL OUR BRAND SPECIALISTS TODAY TO SEE HOW WE CAN HELP ROYALMFG.COM
GARY KNUTSON: 918-510-4181
- 61 NLGI SPOKESMAN, MARCH/APRIL 2018
AL PARRISH: 601-209-9474
Industry Calendar of Events 2018 Please contact Denise if there are meetings/conventions you’d like to add to our Industry Calendar. firstname.lastname@example.org (Your company does not have to be an NLGI member to post calendar items.)
April 19 – 21 ILMA Management Forum Fort Lauderdale Marriott Harbor Beach Resort & Spa Fort Lauderdale, FL
April 21 – 24 ELGI Annual General Meeting Grange St.Paul’s Hotel London, United Kingdom
May 20 – 24 STLE Annual Meeting & Exhibition Minneapolis Convention Center Minneapolis, MN
June 9 – 12 NLGI 85th Annual Meeting The Coeur d’Alene Resort Coeur d’Alene, ID
October 6 – 9 ILMA Annual Meeting JW Marriott Desert Springs Resort & Spa Palm Desert, CA
- 62 VOLUME 82, NUMBER 1
- 63 NLGI SPOKESMAN, MARCH/APRIL 2018
Servo Filling Systems
Advertiser’s Index Covenant Engineering, page 62 Frigmaires, page 5 Lubes ‘n’ Greases, back cover Monson, page 64 Patterson Industries Canada, page 63
Petro-Lubricant Testing Laboratories, Inc, page 5 ProSys, page 65 Royal Manufacturing, page 61 Vanderbilt Chemicals LLC, Inside Front Cover - 65 NLGI SPOKESMAN, MARCH/APRIL 2018
WE GET TO THE HEART OF A COMPLEX INDUSTRY. www.LubeReportAsia.com A critical weekly roundup of the lubricant industry in Asia. Featuring breaking news and base oil price reports in English and Simplified Chinese.
www.LubeReport.com The weekly e-newsletter containing late-breaking and trending industry news; base oil price reports for North America, Europe, Middle East and Africa; and regional shipping report.
Lubes’n’Greases Magazine Covering the global issues, trends and news that affect your success.
Lubes’n’Greases EMEA Magazine Offering a focused look at Europe, Middle East, Africa, Russia and more.
GET YOUR SUBSCRIPTIONS TODAY